Author
paulo-sabino
View
67
Download
3
Embed Size (px)
1 F o r m u l a s o f R h e o l o g y
One of the most important steps in processing polymers is melting the resin, which isinitially in the solid state, and forcing the melt through a die of a given shape. During thisoperation, the melt, whose structure plays a key role in determining the quality of theproduct to be manufactured, undergoes different flow and deformation processes.
The plastics engineer has therefore to deal with the melt rheology, which describes the flowbehavior and deformation of the melt. The theory of elasticity and hydromechanics canbe considered the frontier field of rheology, because the former describes the behavior ofideal elastic solids, whereas the latter is concerned with the behavior of ideal viscous fluids.
Ideal elastic solids deform according to Hooke's Law and ideal viscous fluids obey thelaws of Newtonian flow. The latter are also denoted as Newtonian fluids. Plastic meltsexhibit both viscous and elastic properties.
Thus, the design of machines and dies for polymer processing requires quantitativedescription of the properties related to polymer melt flow. Starting from the relationshipsfor Hookean solids, formulas describing viscous shear flow of the melt are treated first,as far as they are of practical use in designing polymer machinery. This is followed by asummary of expressions for steady and time-dependent viscoelastic behavior of melts.
1.1 Idea l So l ids
The behavior of a polymer subjected to shear or tension can be described by comparingits reaction to external force with that of an ideal elastic solid under load. To characterizeideal solids, first of all it is necessary to define certain quantities as follows [I]:
The axial force Fn in Figure 1.1 causes an elongation A/ of the sample of diameter dQ andlength I0 that is fixed at one end. Following equations apply for this case:
Engineering strain:
Hencky strain:
Tensile stress:
(Li)
(1.2)
(1.3)
Figure 1.1 Deformation of a Hookean solid by a tensile stress [1 ]
Reference area:
(1.4)
Poisson's ratio:
Figure 1.2 shows the influence of a shear force Fv acting on the area A of a rectangularsample causing the displacement AU. The valid expressions are defined by:
Shear strain:
(1.5)
Shear stress:
(1.6)
(1.7)
Figure 1.2 Deformation of a Hookean solid by shearing stress [1 ]
VtrbV P
P
Figure 1.3 Hookean solid under compression [1]
The isotropic compression due to the pressure acting on all sides of the cube shown inFigure 1.3 is given by the engineering compression ratio K
where AV is the reduction of volume of a body with the original volume V0 due todeformation.
1.1.1 Hooke'sLaw
The linear relationships between stress and strain of a Hookean solid are given by [I].
(1.8)
(1.9)
(1.10)
(1.11)
Where E is the modulus of elasticity, G is the shear modulus, and K is the bulk modulus.These moduli are constant for a Hookean solid. In addition, the relationship existingbetween £, G and K is expressed as [ 1 ]
For an incompressible solid this leads (K —»<*>, jl —> 0.5) to [1]
E = 3G
(1.12)
(1.13)
1.2 Newton ian Fluids
There is a linear relationship between stress and strain in the case of Newtonian fluidssimilar to the one for ideal elastic solids.
The fluid between the upper plate in Figure 1.4 is moving at a constant velocity Ux andthe lower stationary plate experiences a shear stress T (see also Figure 1.2).
Figure 1.4 Shear flow
(1.14)
The shear or deformation rate of the fluid is equal to
(1.15)
The shear viscosity is defined as
(1.16)
For an extensional flow, which corresponds to the tension test of a Hookean solid, we get
(1.17)
where
<TZ = normal stressX = Trouton viscosity£ - strain rate
Analogously to Equation 1.13 one obtains
(1.18)
1.3 Formulas for Viscous Shear Flow of Polymer Mel ts
Macromolecular fluids such as thermoplastic melts exhibit significant non-Newtonianbehavior. This can be seen in the marked decrease of melt viscosity when the melt issubjected to shear or tension as shown in Figure 1.5. The plastic melt in the channels ofpolymer processing machinery is subjected mainly to shear flow. Therefore, knowledgeof the laws of shear flow is necessary when designing machines and dies for polymerprocessing. For practical applications, the following summary of the relationships wasfound to be useful.
y
x
Ux
H
Figure 1.5 Tensile viscosity and shear rate viscosity of a polymer melt as a function of strain rate [21 ]
13.1 Apparent Shear Rate
The apparent shear rate for a melt flowing through a capillary is defined as
(1.19)
where Q is the volume flow rate per second and £ is the radius of the capillary.
1.3.2 Entrance Loss
Another rheological quantity of practical importance is the entrance losspc, representingthe loss of energy of flow at the entrance to a round nozzle. This is empirically correlatedby the relation [2]
(1.20)
Table 1.1 Resin-Dependent Constants c and m in Equation 1.20 [2]
Polymer
Polypropylene (Novolen 1120 H)Polypropylene (Novolen 1120 L)Polypropylene (Novolen 1320 L)
LDPE (Lupolen 1800 M)LDPE (Lupolen 1800 S)LDPE (Lupolen 1810 D)
HDPE (Lupolen 6011 L)HDPE (Lupolen 6041 D)
Polyisobutylene (Oppanol B 10)Polyisobutylene (Oppanol B 15)
C
2.551 • 10"5
1.463 • 10"1
2.871 • 10~7
1.176- 10"1
6.984 • 10°5.688 • 10^
3.940 • 10"2
1.778 • 10°
6.401 • 10"3
1.021 • 10"7
m
2.1161.9762.469
1.4341.0721.905
1.3991.187
1.5752.614
igeo.ig*-
ig*M
g/*
/ V ^ o
where c and m are empirical constants and T is the shear stress. These constants can bedetermined from the well-known Bagley-curves as shown in Figure 1.7. The values ofthese constants are given in Table 1.1 for some thermoplastic materials. Shear stress andentrance loss are measured in Pa in the calculation of c and m.
1.3.3 True Shear Stress
The flow curves of a particular LDPE measured with a capillary rheometer are given inFigure 1.6. The plot shows the apparent shear rate J as a function of the true shear stressT at the capillary wall with the melt temperature as a parameter. The entrance loss pc wasobtained from the Bagley plot shown in Figure 1.7.
Shea
r rate
f
Pres
sure
p
Figure 1.6 Flow curves of a LDPE [8]Shear stress T
S"1
Pa
T-- 23O0C
19O0C
15O0C
#=1mm= 0,6 mm
bar
Figure 1.7 Bagley plots of a polystyrene with the capillary length L and radius R [3]Capillary geometry L/R
Thus, the true shear stress T is given by
(1.21)
where
L = length of the capillaryR = radius of the capillaryp = pressure of the melt (see Figure 1.39).
1.3.4 Apparent Viscosity
The apparent viscosity 7]a is defined as
(1.22)
and is shown in Figure 1.8 as a function of shear rate and temperature for a LDPE.
Shear rate f
Figure 1.8 Viscosity functions of a LDPE [8]
1.3.5 True Shear Rate
The t rue shear rate yt is obtained from the apparent shear rate by applying the correctionfor the n o n Newtonian behavior of the melt according to Rabinowitsch
(1.23)
The meaning of the power law exponent n is explained in the Section 1.3.7.2.
Visc
osity
7\
s"1
Pa-s
Figure 1.9 True and apparent viscosity functions of a polystyrene at different temperatures [2]
1.3.6 True Viscosity
The true viscosity T]w is given by
(1.24)
In Figure 1.9, the true and apparent viscosities are plotted as functions of the correspond-ing shear rates at different temperatures for a polystyrene. As can be seen, the apparentviscosity function is a good approximation for engineering calculations.
1.3.7 Empirical Formulas for Apparent Viscosity
Various fluid models have been developed to calculate the apparent shear viscosity 7]a
[9]. The following sections deal with some important relationships frequently used indesign calculations.
1.3.7.1 Hyperbolic Function of Prandtl and Eyring
The relation between shear rate % and shear stress T according to the fluid model ofEYRING [4] and PRANDTL [5] can be written as
(1.25)
where C and A are temperature-dependent material constants.
The evaluation of the constants C and A for the flow curve of LDPE at 190 0C in Figure 1.10leads to C = 4 s"1 and A = 3 • 104 N/m2. It can be seen from Figure 1.10 that the hyperbolicfunction of Eyring and Prandtl holds good at low shear rates.
Apparent shear rate fQTrue shear rate fx
Appa
rent v
iscos
ity 7
\ QTr
ue v
iscos
ity 7
fo
PQ-S Polystyrene
s"1
Shear stress rFigure 1.10 Comparison between measurements and values calculated with Equation 1.25 [8]
1.3.7.2 Power Law of Ostwald and de Waele
The power law of OSTWALD [6] and DE WAELE [7] is easy to use, hence widely employed indesign work [10]. This relation can be expressed as
(1.26)
(1.27)
where K denotes a factor of proportionality and n the power law exponent. Anotherform of power law often used is
(1.28)
(1.29)
In this case, nR is the reciprocal of n and KR = K~nR . From Equation 1.26 the exponentn can be expressed as
or
or
N/m2
Shea
r ra
te f
s"1
(1.30)
PE-LD19O0C
Shear stress TFigure 1.11 Determination of the power law exponent n in Equation 1.30
As shown in Figure Ll 1, in a double log plot the exponent n represents the local gradientof the curve y^ vs. T.
Furthermore
(1.31)
The values of K and n determined from the flow curve of LDPE at 190 0C shown inFigure 1.12 were found to be K = 1.06 • 10"11 and n = 2.57 [8]. As can be seen fromFigure 1.12, the power law fits the measured values much better than the hyperbolicfunction of EYRING [4] and PRANDTL [5]. The deviation between the results from the powerlaw and from the experiment is a result of the assumption that the exponent n is constantthroughout the range of shear rates considered, whereas in fact n varies with the shearrate. The power law can be extended to consider the effect of temperature on the viscosityas follows:
(1.32)
where
K0R = consistency indexP = temperature coefficientT = temperature of melt.
Shea
r rate
f
s"1 PE-LDr=150°C
t a n a = d l ^ = / 7
Pa
Shear stress TFigure 1.12 Comparison between measured values and power law
Example
Following values are given for a LDPE:
nR = 0.3286
J3 =0.00863 (0C"1)
KOR =135990 (N s"R • nT2)
The viscosity 7]a at T = 200 0C and ya = 500 s"1 is calculated from Equation 1.32
7JZ = 373.1Pa-s
1.3.7.3 Muenstedt's Polynomial
The fourth degree polynomial of MUENSTEDT [2] provides a good fit for the measuredvalues of viscosity. For a specific temperature this is expressed as
(1.33)
where A0, A1, A2, A3, A4 represent resin-dependent constants. These constants can bedetermined with the help of the program of RAO [ 10], which is based on multiple linearregressions.
This program in its general form fits an equation of the type
and prints out the coefficients a0, ax and so on for the best fit.
Shea
r ra
te y
s"1
N/m2
measured
PE-LO19O0C
Shift Factor for Crystalline Polymers
The influence of temperature on viscosity can be taken into account by the shift factor aT
[2].
For crystalline polymers this can be expressed as
(1.34)
where
bv b2 = resin dependent constantsT = melt temperature (K)T0 - reference temperature (K)
Shift Factor for Amorphous Polymers
The shift factor aT for amorphous polymers is derived from the WLF equation and canbe written as
(1.35)
where
C1, C2 = resin dependent constantsT = melt temperature (0C)T0 = reference temperature (0C)
The expression for calculating both the effect of temperature and shear rate on viscosityfollows from Equation 1.33.
(1.36)
With Equation 1.31 we get
(1.37)
The power law exponent is often required in the design work as a function of shear rateand temperature. Figure 1.13 illustrates this relationship for a specific LDPE. The curvesshown are computed with Equation 1.34 and Equation 1.37. As can be inferred fromFigure 1.13, the assumption of a constant value for the power law exponent holds goodfor a wide range of shear rates.
Figure 1.13 Power law exponent of a LDPE as a function of shear rate and temperature
Example
The viscosity for a LDPE is to be calculated with the following constants:
A = 4.2541Al = -0.4978A2 = -0.0731A3= 0.0133A 4 - -0.0011B = 5.13 -10"6
Bl = 5640K
at Y^ = 500 s"1 and T = 200 0C.
Solution
aT from Equation 1.34
Powe
r law
exp
onen
t n
Shear rate fs-1
PE-LD
With
7]a from Equation 1.36
Substituting the values of A0, A1, and so on yields
The power law exponent is obtained from Equation 1.37
Using the values for A0, A v and so on
n = 3.196
1.3.7.4 Carreau's Viscosity Equation [11]
As shown in Figure 1.14 [12], the Carreau equation provides the best fit for the viscosityfunction, reproducing the asymptotic form of the plot at high and low shear rates correctly.
The equation is expressed as
(1.38)
where A, B, C are resin-dependent constants. By introducing the shift factor aT intoEquation 1.38, the temperature-invariant form of the Carreau equation can be given as
(1.39)
For a number of resins the shift factor can be calculated as a function of temperaturefrom the following equation with good approximation [9,10]
(1.40)
where T1 (0C) is the temperature at which the viscosity is given and T2 (
0C) the temperatureat which the viscosity is calculated.
The standard temperature TST is given by [9]
TST=Tg +500C (1.41)
Visc
osity
7?
Figure 1.14 Determination of Carreau-parameters from a viscosity function [12]
Shear rate f
Slope: -CVo=*
/=1/B
Data on typical glass transition temperatures of polymers are given in Table 3.1 [9].
The power law exponent n can be obtained from Equation 1.39:
(1.42)
For high shear rates n becomes [12]
1n =
1 - C
Example
Following constants are given for a specific LDPE:
A = 32400 Pa • sB = 3.1sC = 0.62TST = -133 0CT1 = 1900C
The viscosity is to be calculated at
T2 = 200 0C and fa = 500 s"1.
Solution
From Equation 1.40 one obtains
and
The power law exponent is calculated from Equation 1.42
where
1.3.7.5 Klein's Viscosity Formula [14]
The regression equation of Klein et al. [14] is given by
(1.43)
T = temperature of the melt (0F)?7a = viscosity (lbf • s/in2)
The resin-dependent constants a0 to a22 can be determined with the help of the computerprogram given in [10], as in the case of the A-coefficients in Equation 1.33.
Example
Following constants are valid for a specific type of LDPE. What is the viscosity ?7a atya =500s"1 and T = 200 0C?
a0 = 3.388U1 = -6.351 -10"1
an = -1.815 -10~2
a2 = -5.975 -10"3
a22 =-2.51 • lO^andal2 = 5.187- 10"4
Solution
T (0F) = 1.8 • T (°C)+32 = 1.8 • 200 + 32 = 392
With the constants above and Equation 1.43 one gets
and in Si-units
77a = 6857 • 0.066 = 452.56 Pa • s
The expression for the power law exponent n can be derived from Equation 1.31 andEquation 1.43. The exponent n is given by
(1.44)
Putting the constants ax ... an into this equation obtains
n = 2.919
1.3.7.6 Effect of Pressure on Viscosity
Compared to the influence of temperature, the effect of pressure on viscosity is of minorsignificance.
However, the relative measure of viscosity can be obtained from [9,15,16]
(1.45)
where
rjp = viscosity at pressure p and constant shear stress T0
T]0 = viscosity at constant shear stress T0
ap = pressure coefficient
For styrene polymers rjp is calculated from [14]
">=thespkL) (L46)
where p - pressure in bar.
Thus the change of viscosity with pressure can be obtained from Equation 1.46. Table 1.2shows the values of viscosity calculated according to Equation 1.46 for a polystyrene ofaverage molecular weight. It can be seen that a pressure of 200 bar causes an increase ofviscosity of 22% compared to the value at 1 bar. The pressure coefficient of LDPE is lessthan that of PS by a factor of 3-4 and the value of HDPE is again smaller by a factor of 2compared to LDPE. This means that in the case of polyethylene an increase of pressureby 200 bar would enhance the viscosity only by 3 to 4%. Consequently, the effect ofpressure on viscosity can be neglected in the case of extrusion processes which generallyuse low pressure. However, in injection molding with its high pressures, typically thedependence of viscosity on pressure has to be considered.
1.3.7.7 Dependence of Viscosity on Molecular Weight
The relationship between viscosity and molecular weight can be described by [12]
(1.47)
Table 1.2 Effect of Pressure on Viscosity for Polystyrene, Equation 1.46
Pbar
30100200300500
10003000
1.03 TJ0
1.105 TJ0
1.221 TJ0
1.35 TJ0
1.65 TJ0
2.72 TJ0
2 0 TJ0
where
Mw = molecular weight
JC — resin dependent constant
The approximate value of JC for LDPE is
JC = 2.28 • 10"4
and for polyamide 6
K'= 5.21 • 10"14
according to the measurements of LAUN [21].
These values are based on zero viscosity.
1.3.7.8 Viscosity of Two Component Mixtures
The viscosity of a mixture consisting of a component A and a component B can beobtained from [17]
(1.48)
where
7] = viscosityC = weight per cent
Indices:
M: mixtureAy B: components
1.4 Viscoelastic Behavior of Polymers
Polymer machinery can be designed sufficiently accurately on the basis of the relationshipsfor viscous shear flow alone. However, a complete analysis of melt flow should includeboth viscous and elastic effects, although the design of machines and dies is rather difficultwhen considering melt elasticity and therefore rarely used. WAGNER [18] and FISCHER
[19] made attempts to dimension dies taking elastic effects into account.
For a more complete picture of melt theology the following expressions for the viscoelasticquantities according to LAUN [20, 21] are presented. The calculation of the deformationof the bubble in film blowing is referred to as an example of the application of Maxwell'smodel.
1.4.1 Shear
1.4.1.1 Linear Viscoelastic Behavior
The linear viscoelastic behavior occurs at low shear rates or small shear.
Steady Shear Flow
Zero viscosity T]0 as a material function for the viscous behavior (Figure 1.15 and 1.16):
(1.49)
Figure 1.15 Time dependence of shear strain and shear stress in a stress test at constant shear rateY0 and subsequent recoil due to unloading (shear stress T= 0) with yrs as recoverableshear strain [21]
Time /Figure 1.16 Creep test at constant shear stress T0 and subsequent retardation after unloading
(shear stress T=O) [20].yrs = recoverable shear strain; I = initial state; Il = steady state; III = retardation
Shea
r j
Shea
r str
ess T
Shea
r str
ess T
Shea
r y
Time/
I II III
T0
I II III
T0
Steady state shear compliance J°t (Figure 1.15 and Figure 1.16) as a characteristicparameter for the elastic behavior:
(1.50)
Time-dependent Behavior
OViscosity Tj(t) (Figure 1.17):
(1.51)
OShear compliance J(t) (Figure 1.18):
(1.52)
Maximum time of retardation Tmax as a rheological quantity for the transient behavior(Figure 1.19):
(1.53)
Figure 1.17 Initial state in a stress test under linear shear flow [21]
Figure 1.18 Initial state in creep under linear shear flow [21]
igi(
«Ig
J(Z)
ig/
ig7?o
tFigure 1.20 Relaxation after a step shear strain y0 [21 ]
OShear stress relaxation modulus G(t) (Figure 1.20 and Figure 1.21):
(1.54)
Dependence of storage modulus G' and loss modulus G" on frequency (Figure 1.22)with sinusoidal shear strain y.
(1.55)
Sinusoidal and out-of-phase shear stress V.
(1.56)
where
Y = amplitude of shearCO = angular frequency
The storage modulus G'{(0) characterizes the elastic behavior, whereas the loss modulusG" depicts the viscous behavior of the melt subjected to periodic shear deformation.
l9(*, s
-?-r)
7x
Figure 1.19 Retardation from steady shear flow [21] (shear stress T= Oat time f = 0)t
X
t
lga;
Figure 1.22 Storage modulus G and loss modulus G" as functions of frequency
Expressions for conversion:
Determination of zero viscosity and shear compliance from relaxation modulus [21]:
(1.57)
(1.58)
Determination of zero viscosity and shear compliance from storage and loss moduli[21]:
(1.59)
(1.60)
Ig 6\
Ig G"
IgM
/)
Figure 1.21 Relaxation modulus of linear shear flow [21]ig(/)
1.4.1.2 Nonlinear Viscoelastic Behavior
Steady Shear Flow
The viscosity
and the shear compliance
are dependent on the shear rate and shear stress respectively in the nonlinear case. Theirlimiting values for small shear rates or shear stresses are T]0 and J°t (Figure 1.23). Anothermaterial function in addition to the shear compliance characterizing the elastic behavioris the primary normal stress coefficient 0 with Nx as the normal stress difference:
The limiting value of the normal stress function @(/0) (Figure 1.23) at low shear rates is
given by
G0 = lim S(Yo) (1-62)yo->O
In addition, we have:
igJe
.lg7?,
ig®
Figure 1.23 Parameters for steady shear flow [21]. I = linear region; Il = nonlinear region
(1.63)
III
(1.61)
Characterization of the Transient State
Initial state in a stress test (Figure 1.24)
(1.64)O7]{t) is the asymptote.
Plots of starting state in creep test (Figure 1.25)
(1.65)0
J(t) is the asymptote.
Relaxation modulus (Figure 1.26):
(1.66)
The time-dependent behavior remains unchanged in the nonlinear case. The entirefunction plot will be displaced by the factor H(YQ).
Ig n
(t)
IgJ(
M
Figure 1.25 Initial state in creep test of nonlinear shear flow [21 ]
Ig/
Figure 1.24 Initial state in a stress test of nonlinear shear flow [21]
Ig/
T0
Figure 1.26 Relaxation modulus of nonlinear shear flow [21]
1.4.2 Uniaxial Tension
1.4.2.1 Linear Viscoelastic Behavior
Steady Tensile Extensional Flow
Tensile zero viscosity /J0 as a material function for the viscous behavior (Figure 1.27 andFigure 1.28)
(1.67)
Steady state tensile compliance D° as a material function for elastic behavior:
Stra
in E
Tens
ile s
tress
6IQ
Git)
(1.68)
Time /
Time /Figure 1.27 Time dependence of tensile strain and tensile stress at constant tensile strain rate S0
and subsequent retardation after unloading (tensile stress T= 0) [2].£rs = recoverable tensile strain; I = initial state; Il = steady state; III = retardation
I II III
Time/Figure 1.28 Tensile creep at constant tensile stress T0 and subsequent retardation after unloading
(tensile stress T=O) [21]
Transient Behavior
Tensile viscosity ju(t) (Figure 1.29)
(1.69)
(1.70)
The tensile viscosity is three times the shear viscosity.O
Tensile creep compliance D(t) (Figure 1.30):
(1.71)
(1.72)
Maximum retardation time Tmax (Figure 1.31)
(1.73)
Relaxation after a step strain of £0:O
Tensile relaxation modulus E(t) (Figure 1.32):
Tens
ile s
tress
6St
rain e
Time t-
I n in
IgAC
/)lg
/?(/)
lg(e
riS-e
r)ig
/fV)
Mo
Ig/Figure 1.29 Initial state of linear tensile extension [21]
Ig/
Time /Figure 1.31 Retardation from steady state tensile extension [21]
Figure 1.32 Tensile relaxation modulus of tensile extensional flow [21]
Ig/
Figure 1.30 Initial state in tensile creep under linear tensile extension [21]
JL
">I-TU
1.4.2.2 Nonlinear Viscoelastic Behavior
Steady Tensile Extensional Flow
As shown in Figure 1.5, the tensile viscosity /a is given by
Tensile compliance De (Figure 1.33)
Figure 1.33 Plot of tensile compliance D6 and shear compliance Je [21]
Time-dependent Behavior
Plots of starting state in tension test (Figure 1.34) [21]
(1.76)0ju(t) is an asymptote.
Start-up curves in a tensile creep test (Figure 1.35) [21]
(1.77)0D(t) is an asymptote.
Tensile relaxation modulus (Figure 1.36)
(1.78)
(1.74)
(1.75)
ig4.
W
Ig f
Wiq
D(t)
\Qfil
t)
Figure 1.36 Tensile relaxation modulus as a function of time under nonlinear tensile extension [21]
1.43 Maxwell Model
The viscoelastic properties of a polymer can be used to calculate the deformation of abubble in a film blowing process. In this case, the Maxwell model, which defines aviscoelastic body as an ideal spring and a dashpot in series (Figure 1.37) can be applied[18,19].
Ig/Figure 1.35 Initial state of tensile creep under nonlinear extension [21 ]
Ig/Figure 1.34 Initial state of nonlinear tensile extension [21]
Figure 1.37 Maxwell fluid [1 ]
The total rate of deformation y is the sum of the elastic component yu and viscouscomponent ^N
(1.79)
(1.80)
(1.81)
The time ts is called the relaxation time, as the stress T relaxes with the time.
77H = Newtonian viscosityGH = elastic shear modulus of the spring (Hooke element)
At a given rate of deformation, the viscosity % s reaches the Newtonian value asympto-tically (Figure 1.38). After the release of strain the stress delays according to
(1.82)
It can be seen from Equation 1.82 that the relaxation time is the period, in which thestress decreases to lie (37%) of its original value [23]. It also follows from Equation 1.82that the modulus of relaxation G for y— yQ is given by
7JM1S
(1.83)
tFigure 138 Tensile viscosity of Maxwell fluid [1 ]
where
leading to [22]
F
G*
\
The expression for the elongation of the bubble in a film blowing process can now begiven as
(1.84)
where
<7 = tensile stress,ts = relaxation time,[l = tensile viscosity of the melt,v = vertical velocity component of the bubble,x - axial coordinate.
As the elongation of the bubble occurs biaxially, the deformation in the circumferentialdirection has to be calculated on similar lines. Assuming that the tensile viscosities andthe relaxation times in both directions are equal, the influence of viscoelasticity on thebubble form can be predicted [18]. WAGNER [18] estimates the relaxation time in theorder of 5 to 11 s, depending on the operating conditions.
1.4.4 Practical Formulas for Die Swell and Extensional Flow
Elastic effects are responsible for die swell, which occurs when the melt exits through adie as shown in Figure 1.39 [20].
The following equation for the die swell is given by COGSWELL [24]:
(1.85)
where
BL = die swell — (Figure 1.39) in a capillary with a length-to-diameter ratio^o greater than 16 and
/R = recoverable shear strain
In Figure 1.40, the recoverable shear strain is presented as a function of die swell accordingto Equation 1.85 [24].
Figure 1.39 Die swell in extrusion
\P
d
L do
Die swell B1
Figure 1.40 Dependence of recoverable shear on die swell [24]
Extensional Flow
The following relationships for extensional flow of melt after COGSWELL [24] are importantin practice:
Elongational stress <TE:
(1.86)
(1.87)
(1.88)
(1.89)
where
= reciprocal of power law index n in Equation 1.28= entrance pressure loss according to Equation 1.20= apparent shear rate and apparent shear viscosity, respectively= die swell in melt flow through an orifice with zero length
Reco
verab
le sh
ear /
R
Tensile viscosity fl:
Reversible extension £R
Rupture stress <7R
References
[I] PAHL, M., BALDHUHN, R., LINNEMANN, D.: Praktische Rheologie der Kunststoffschmelzen and
Losungen, VDI Kunststofftechnik, Dusseldorf (1982)
[2] MONSTEDT, H.: Kunststoffe 68, 92 (1978)
[3] Kunststoff Physik im Gesprach, brochure, BASF, 1977
[4] EYRING, H.: I. Chem. Phys. 4, 283 (1963)
[5] PRANDTL, L.: Phys. Blatter 5,161 (1949)
[6] OSTWALD, W.: Kolloid Z. 36, 99 (1925)
[7] DE WAALE, A.: /. Oil and Color Chem. Assoc. 6, 33 (1923)
[8] RAO, N. S.: Berechnen von Extrudierwerkzeugen, VDI Verlag, Dusseldorf (1978)
[9] RAUWENDAAL, C : Polymer Extrusion, Hanser Publishers, Munich (2001)
[ 10] RAO, N. S.: Designing Machines and Dies for Polymer Processing with Computer Programs,Hanser Publishers, Munich (1981)
[II] CARREAU, P. J.: Dissertation, Univ. Wisconsin, Madison (1968)
[12] HERTLEIN, T., FRITZ, H. G.: Kunststoffe 78, 606 (1988)
[13] MiCHAELi, W.: Extrusion Dies, Hanser Publishers, Munich (2003)
[14] KLEIN, L, MARSHALL, D. L, FRIEHE, C. A.: /. Soc. Plastics Engrs. 21,1299 (1965)
[15] AVENAS, P., AGASSANT, J. E, SERGENT, J.PH.: La Mise en Forme des Matieres Plastiques, Technique
& Documentation (Lavoisier), Paris (1982)
[16] MONSTEDT, H.: Berechnen von Extrudierwerkzeugen, VDI Verlag, Dusseldorf (1978)
[ 17] CARLEY, J. E: Antec 84, S. 439
[18] WAGNER, M. H.: Dissertation, Univ. Stuttgart (1976)
[19] FISCHER, E.: Dissertation, Univ. Stuttgart (1983)
[20] LAUN, H. M.: Rheol. Acta 18,478 (1979)
[21] LAUN, H. M.: Progr. Colloid & Polymer ScL 75, 111 (1987)
[22] BRYDSON, J. A.: Flow Properties of Polymer Melts, Iliffe Books, London (1970)
[23] BERNHARDT, E. C : Processing of Thermoplastic Materials, Reinhold, New York (1963)
[24] COGSWELL, F. N.: Polymer Melt Rheology, John Wiley, New York (1981)
2 T h e r m o d y n a m i c P r o p e r t i e s o f P o l y m e r s
In addition to the rheological data, thermodynamic properties of polymers are necessaryfor designing machines and dies. It is often the case that the local values of these data arerequired as functions of temperature and pressure. Besides physical relationships, thischapter presents regression equations developed from experimental data for calculatingthermodynamic properties, as these polynomials are often used in the practice, forexample, in data acquisition for data banks [I].
2.1 Speci f ic V o l u m e
According to the Spencer Gilmore equation, which is similar to the van der Waal equationfor real gases, the relationship between pressure p, specific volume v, and temperature Tof a polymer can be written as
(2.1)
In this equation, b is the specific individual volume of the macromolecule, p is thecohesion pressure, W is the molecular weight of the monomer, and R is the universal gasconstant [2].
Example
Following values are given for a LDPE:
W = 28.1 g/Mol;b\ = 0.875 cm3/g;p =3240atm
Calculate the specific volume v at T = 190 0C andp = 1 bar.
Solution
Using Equation 2.1 and the conversion factors to obtain the volume v in cm3/g, we obtain
The density p is the reciprocal value of the specific volume so that
(2.2)
Temperature T
Figure 2.1 Specific volume as a function of temperature and pressure for LDPE [1 ]
The functional relationship between specific volume v, pressure p, and temperature Tcan also be expressed by a polynomial of the form [1,3]
(2.3)
if experimental data are available (Figure 2.1). The empirical coefficients A(0)v ... A(3)v
can be determined by means of the computer program given in [ 1].
2.2 Specific Heat
The specific heat cp is defined as
(2.4)
where
h = EnthalpyT — Temperature
The specific heat cp defines the amount of heat that is supplied to a system in a reversibleprocess at a constant pressure to increase the temperature of the substance by dT.
The specific heat at constant volume cv is given by
Spec
ific v
olume
v
cm3/g
0C
measuredpolynomial
800 bar
400 bar
/>=1bar
(2.5)
where
u = internal energyT = temperature
In the case of cv the supply of heat to the system occurs at constant volume.
cp and cv are related to each other through the Spencer-Gilmore equation (Equation 2.1):
(2.6)
The numerical values of cp and cv differ by roughly 10%, so that for approximate calcu-lations cv can be considered equal to cp [2].
Plots of cp as a function of temperature are shown in Figure 2.2 for amorphous,semicrystalline, and crystalline polymers.
As shown in Figure 2.3, the measured values can be expressed by a polynomial of thetype
Spec
ific h
eat C
p
(2.7)
a) b) c)
Figure 2.2 Specific heat as a function of temperature for amorphous (a), semi crystalline (b),and crystalline polymers (c) [4]
/mh
kg K
Figure 2.3 Comparison between measured values of cp [6] and polynomial for LDPE [1]Temperature J
0C
polynomialmeasured
The use of thermal properties cp and p in design problems is illustrated in the examplesgiven in Chapter 6.
The expansion coefficient O^ at constant pressure is given by [4]
(2.8)
The linear expansion coefficient Ce11n is approximately
(2.9)
The isothermal compression coefficient yK is defined as [4]
(2.10)
av and yK are related to each other by the expression [4]
(2.11)
2.3 Enthalpy
Equation 2.4 leads to
(2.12)
As shown in Figure 2.4, the measured data on h = h(T) [6] for a polymer melt can beexpressed by the polynomial
(2.13)
The specific enthalpy defined as the total energy supplied to the polymer divided bythroughput of the polymer is a useful parameter for designing extrusion and injectionmolding equipment such as screws. It provides the theoretical amount of energy requiredto bring the solid polymer to the process temperature.
Values of this parameter for different polymers are given in Figure 2.5 [4].
If, for example, the throughput of an extruder is 100 kg/h of polyamide (PA) and theprocessing temperature is 260 0C, the theoretical power requirement would be 20 kW.This can be assumed to be a safe design value for the motor horse power, althoughtheoretically it includes the power supply to the polymer by the heater bands of theextruder as well.
Entha
lpy
/7-/72
0
Figure 2.5 Specific enthalpy as a function of temperature [4]
Temperature T
0C
PVC
PA PSPC
kWhkg
Temperature TFigure 2.4 Comparison between measured values of/? [6] and polynomial for PA-6 [I]
0C
Klkg polynomial
measured
2.4 Thermal Conduct iv i ty
The thermal conductivity X is defined as
(2.14)
where
Q = heat flow through the surface of area A in a period of time t(T1-T2) = temperature difference over the length /
Analogous to the specific heat cp and enthalpy h, the thermal conductivity X can beexpressed as [1]
(2.15)
as shown in Figure 2.6.
Temperature TFigure 2.6 Comparison between measured values of X [6] and polynomial for PP [1 ]
The thermal conductivity increases only slightly with pressure. A pressure increase from1 bar to 250 bar leads to an increase of only less than 5% of its value at 1 bar.
Within a particular resin category such as LDPE, HDPE, the thermal properties are largelyindependent of the molecular structure. Exhaustive measured data of the quantities cp,hy and X and pressure-volume-temperature diagrams of polymers are given in the VDMA-Handbook [5].
Approximate values of thermal properties useful for plastics engineers are summarizedin Table 2.1 [4].
Therm
al co
nduc
tivity
A
0C
mKmeasured
polynomial
References
[ 1 ] RAO, N. S.: Designing Machines and Dies for Polymer Processing, Hanser Publishers, Munich(1981)
[2] KALIVODA, P.: Lecture, Seminar: Optimieren von Kunststofrmaschinen und -werkzeugen mitEDV, Haus der Technik, Essen (1982)
[3] MUNSTEDT, H.: Berechnen von Extrudierwerkzeugen, VDI-Verlag, Diisseldorf (1978)
[4] RAUWENDAAL, C : Polymer Extrusion, Hanser Publishers, Munich (2001)
[5] Kenndaten fur die Verarbeitung thermoplastischer Kunststoffe, Teil I, Thermodynamik,Hanser Publishers, Munich (1979)
[6] Proceedings, 9. Kunststofftechnisches Kolloquium, IKV, Aachen (1978), p. 52
Table 2.1 Approximate Values for the Thermal Properties of Selected Polymers [4]
Polymer
PSPVCPMMASANABSPCLDPELLDPEHDPEPPPA-6PA-6.6PETPBT
Thermalconductivity
XW/m K
0.120.210.200.120.250.190.240.240.250.150.250.240.290.21
Specific heat
CP
kJ/kgK
1.201.101.451.401.401.402.302.302.252.102.152.151.551.25
Density
P 3g/cm3
1.061.401.181.081.021.200.920.920.950.911.131.141.351.35
Glass transitiontemperature
0C
10180
105115115150
-120/-90-120/-90-120/-90
-1050557045
Meltingpoint range
Tm0 C
ca. 110ca. 125ca. 130
160-170215-225250-260250-260ca. 220
3 F o r m u l a s o f H e a t T r a n s f e r
Heat transfer and flow processes occur in the majority of polymer processing machineryand often determine the production rate. Designing and optimizing machine elementsand processes therefore require knowledge of the fundamentals of these phenomena.The flow behavior of polymer melts has been dealt with in Chapter 2. In the presentchapter, the principles of heat transfer relevant to polymer processing are treated andexplained with examples.
3.1 S teady S ta te C o n d u c t i o n
Fourier's law for one-dimensional conduction is given by
(3.1)
where
Q = heat flow thermal conductivityA — area perpendicular to the direction of heat flowT = temperaturex = distance (Figure 3.1)
(3.2)
(3.3)
Figure 3.1 Plane wall [1]
3.1.1 Plane Wall
Temperature profile (Figure 3.1) [I]:
Heat flow:
Analogous to Ohm's law in electric circuit theory, Equation 3.3 can be written as [2]
(3.4)
(3.5)
where
AT = temperature difference8 — wall thicknessjR = thermal resistance
Example
The temperatures of a plastic sheet (30 mm thick) with a thermal conductivity X =0.335 W/(m K) are TWi = 100 0C and TWi = 40 0C accordingto Figure 3.1. Calculate theheat flow per unit area of the sheet.
Solution
Substituting the given values in Equation 3.3 we obtain
3.1.2 Cylinder
Temperature distribution (Figure 3.2) [I]:
Figure 3.2 Cylindrical wall [1]
(3.6)
in which
Heat flow:
(3.7)
with the log mean surface area A1n of the cylinder
(3.8)
where S= T2-T1.
3.13 Hollow Sphere
Temperature distribution [I]:
(3.9)
with the boundary conditions
Heat flow:
(3.10)
The geometrical mean area Am of the sphere is
(3.11)
The wall thickness S is
(3.12)
3.1.4 Sphere
Heat flow from a sphere in an infinite medium (T2-*00) [1]
(3.13)
where T00 = temperature at a very large distance.
Figure 3.3 shows the temperature profiles of the one-dimensional bodies treated aboveen.
Figure 3.3 One-dimensional heat transfer [1 ] a: sphere, b: cylinder, c: plate
3.1.5 Heat Conduction in Composite Walls
Following the electrical analogy, heat conduction through a multiple layer wall can betreated as a current flowing through resistances connected in series. With this conceptwe obtain for the heat flow through the composite wall as shown in Figure 3.4
(3.14)
(3.15)
(3.16)
Adding Equation 3.14 to Equation 3.16 and setting A1=A2 = A3=A gives
(3.17)
Figure 3.4 Heat transfer through a composite wall [1 ]
Thus
Inserting the conduction resistances
into Equation 3.18 we get
Example 1
A two-layer wall consists of the following insulating materials (see Figure 3.4):
(I1= 16 mm, /^0.048WV(InK)d2 = 140 mm, I2 = 0.033 W/(m K)
The temperatures are Tw = 30 0 C , TWi = 2 0C . Calculate the heat loss per unit area ofthe wall.
Solution
(3.18)
(3.19)
(3.20)
(3.21)
(3.22)
Area A = I m 2
The following example [2] illustrates the calculation of heat transfer through a tube asshown in Figure 3.5.
Figure 3.5 Heat flow in a multilayered cylinder
Example 2
A tube with an outside diameter of 60 mm is insulated with the following materials:
dx = 50 mm, J1 = 0.055 W/(m K)d2 = 40mm, I2 = 0.05 W/(mK)
The temperatures are Tw = 150 0C and TW2 = 30 0C . Calculate the heat loss per unitlength of the tube.
Solution
Resistance R1:
average radius rx:
Resistance R2'-
average radius r2:
Figure 3.6 Heat transfer in composite walls in parallel [1 ]
Heat loss per unit length of the tube according to Equation 3.22:
In the case of multiple-layer walls, in which the heat flow is divided into parallel flows asshown in Figure 3.6, the total heat flow is the sum of the individual heat flows. Thereforewe have
(3.23)
(3.24)
3.1.6 Overall Heat Transfer through Composite Walls
If heat exchange takes place between a fluid and a wall as shown in Figure 3.7, in additionto the conduction resistance we also have convection resistance, which can be written as
(3.25)
where O1 - heat transfer coefficient in the boundary layer near the walls adjacent to thefluids.
Figure 3.7 Conduction and convection through a composite wall [1]
Fluid 1 Fluid 2
The combination of convection and conduction in stationary walls is called overall heattransfer and can be expressed as
(3.26)
where k is denoted as the overall heat transfer coefficient with the corresponding overallresistance Rw
(3.27)
Analogous to conduction for the composite wall in Figure 3.7, the overall resistance JRW
can be given by
(3.28)
(3.29)
A simplified form of Equation 3.29 is
(3.30)
Calculation of the convection heat transfer coefficient is shown in the Section 3.5.
3.2 Transient State Conduct ion
The differential equation for the transient one-dimensional conduction after Fourier isgiven by
(3.31)
where
T = temperaturet = timex = distance
or
The thermal diffusivity a in this equation is defined as
(3.32)
where
X = thermal conductivitycp = specific heat at constant pressurep = density
The numerical solution of Equation 3.31 is given in Section 4.3.4. For commonlyoccurring geometrical shapes, analytical expressions for transient conduction are givenin the following sections.
3.2.1 Temperature Distribution in One-Dimensional Solids
The expression for the heating or cooling of an infinite plate [2] follows from Equation3.31 (Figure 3.8):
(3.33)
(3.34)
where
Tw= constant surface temperature of the plateTa = initial temperatureTb = average temperature of the plate at time tT
tk = heating or cooling timeX = half thickness of the plate [X = -]a, =(n/2)2 2
a = thermal diffusivity, Equation 3.32
Figure 3.8 Non-steady-state conduction in an infinite plate
The Fourier number F0 is defined by
The equation for an infinite cylinder with the radius rm is given by [2]
(3.35)
(3.36)
(3.37)
In the range of F0 > 1, only the first term of these equations is significant. Therefore, forthe heating or cooling time we obtain [2]
Plate:
(3.38)
(3.39)
(3.40)
The solutions of Equation 3.32 to Equation 3.37 are presented in a semi-logarithmicplot in Figure 3.9, in which the temperature ratio 0 ^ = (Tw - Tb)/(TW - Ta) is shownas a function of the Fourier number F0.Not considering small Fourier numbers, these plots are straight lines approximated byEquation 3.38 to Equation 3.40.If the time tk is based on the centre line temperature Th instead of the average temperaturefb, we get [3]
(3.41)
Analogous to Figure 3.9, the ratio 0 ^ with the centre line temperature Tb at time tk isplotted in Figure 3.10 over the Fourier number for bodies of different geometry [4].
Sphere:
Cylinder:
where
and for a sphere with the radius rm
Temp
erat
ure
ratio
6f b
Tem
pera
ture
rat
io &
j b
Fourier number F0
Figure 3.9 Average temperature of an infinite slab (c), a long cylinder (b) and a sphere (a) duringnon-steady heating of cooling [2]
Fourier number F^otZX1
Figure 3.10 Axis temperature for multidimensional bodies [4]
c
b
Q
The foregoing equations apply to cases, in which the thermal resistance between thebody and the surroundings is negligibly small (OC0 -»<*>), for example, in injection moldingbetween the part and the coolant. This means that the Biot number should be very large,Bi —» oo. The Biot number for a plate is
(3.42)
where
aa = heat transfer coefficient of the fluidX = thermal conductivity of the plastic
As the heat transfer coefficient has a finite value in practice, the temperature ratio 0 r
based on the centre line temperature, is given in Figure 3.11 as a function of the Fouriernumber with the reciprocal of the Biot number as parameter [5].
Example 1 [6]
Cooling of a part in an injection mold for the following conditions:
Resin: LDPEThickness of the plate: s =12.7 mmTemperature of the melt: Ta = 243.3 0CMold temperature: Tw = 21.1 0CDemolding temperature: Tb = 76.7 0CThermal diffusivity: a =1.29 10~3 cm2/s
The cooling time tk is to be calculated.
Solution
The temperature ratio 0T b :
Fourier number F0 from Figure 3.10 at 0T b = 0.25
P0 = 0.65
cooling time tk:
Example 2 [6]
Calculate the cooling time tk in Example 1 if the mold is cooled by a coolant with a heattransfer coefficient of aa = 2839 W/(m2 • K).
Solution
As can be extrapolated from Figure 3.11, the Fourier number does not differ much fromthe one in the previous example for &Th = 0.25 and 1/Bi = 0.01342. The resistance dueto convection is therefore negligible and the cooling time remains almost the same.However, the convection resistance has to be taken into account in the case of a film witha thickness of 127 jU that is cooling in quiescent air, as shown in the following calculation:
The heat transfer coefficient for this case is approximately
Example 3 [7]
Cooling of an extruded wire
A polyacetal wire of diameter 3.2 mm is extruded at 190 0C into a water bath at 20 0C.Calculate the length of the water bath to cool the wire from 190 0C to a centre linetemperature of 140 0C. The following conditions are given:
haul-off rate of the wire Vn = 0.5 m/s
P0 from Figure 3.11
F0 = 95
The cooling time
The Biot number Bi
The resulting Biot number is
— = 0.01342Bi
Figure 3.11 Midplane temperature for an infinite plate [5]
Fouri
er nu
mber
F 0=Q
-IZX2
Solution
The Biot number Bi
where R = radius of the wire
The temperature ratio QTh
The Fourier number P0 for QT = 0.706 and —7 = 0.0846 from Figure 3.11 is approxi-mately B i
F0 -0.16
The cooling time tk follows from
fk = 4.1s
The length of the water bath is
3.2.2 Thermal Contact Temperature
If two semi infinite bodies of different initial temperatures 0 A and QAi are broughtinto contact as indicated in Figure 3.12, the resulting contact temperature 0 ^ is givenby [3]
(3.43)
where
= thermal conductivity= density= specific heat= coefficient of heat penetration
— = 0.0846Bi
Bi= 1 7 M - 1 - 6 =11.131000 • 0.23
Figure 3.12 Temperature distribution in semi infinite solids in contact [3]
Equation 3.43 also applies for the case of contact of short duration between thick bodies.It follows from this equation that the contact temperature depends on the ratio of thecoefficients of heat penetration and lies nearer to the initial temperature of body that hasa higher coefficient of penetration. The ratio of the temperature differences (0A - QK)and (0K - QA ) are inversely proportional to the coefficient of penetration:
(3.44)
Example
According to Equation 3.43 [8] the contact temperature Qw of the wall of an injectionmold at the time of injection is
(3.45)
where
= ^J Ape= temperature before injection= melt temperature
Indices w and p refer to mold and polymer, respectively.
As shown in Table 3.1 [8], the coefficients of heat penetration of metals are much higherthan those of polymer melts. Hence the contact temperature lies in the vicinity of themold wall temperature before injection.
The values given in the Table 3.1 refer to the following units of the properties:
thermal conductivity X: W/(m • K)density p: kg/m3
specific heat c: kj/(kg • K)
1 2
/
$
The approximate values for steel are
A =50W/(m-K)p =7850kg/m3
c = 0.485 kj/(kg • K)
The coefficient of heat penetration b
3.3 Heat Conduct ion w i t h Dissipation
The power created by the tangential forces in the control volume of the fluid flow isdenoted as dissipation [9]. In shear flow the rate of energy dissipation per unit volume isequal to the product of shear force and shear rate [ 10]. The power due to dissipation [11]therefore is:
(3.46)
From the power law we get
(3.47)
For a Newtonian fluid with n - 1 we obtain
(3.48)
The applicable differential equation for a melt flow between two plates, where the upperplate is moving with a velocity Ux (Figure 2.4) and the lower plate is stationary [11] is
(3.49)
Table 3.1 Coefficients of Heat Penetration of Mold Material and Resin [8]
Material
Beryllium copper (BeCu 25)Unalloyed steel (C45W3)Chromium steel (X40Crl3)Polyethylene (HDPE)Polystyrene (PS)
Coefficient of heat penetration bWs05Hi2KT1
17.2 • 103
13.8 • 103
11.7- 103
0.99 • 103
0.57 • 103
If the temperature of the upper plate is T1 and that of lower plate is T0, the temperatureprofile of the melt is obtained by integrating Equation 3.51. The resulting expression is
(3.52)
As shown in Section 4.2.3, this equation can be used to calculate the temperature of themelt film in an extruder.
3.4 Dimensionless Groups
Dimensionless groups can be used to describe complicated processes that are influencedby a large number of variables with the advantage that the entire process can be analyzedon a sound basis by means of a few dimensionless parameters. Their use in correlatingexperimental data and in scaling-up of equipment is well known.
Table 3.2 shows some of the dimensionless groups often used in plastics engineering.
Table 3.2 Dimensionless Groups
For drag flow the velocity gradient is given by
Equation 3.49 can now be written as
(3.50)
(3.51)
Symbol
BiBrDeb
F0GrGzLeNaNuPePrReShScSk
Name
Biot numberBrinkman numberDeborah numberFourier numberGrashof numberGraetz numberLewis numberNahme numberNusselt numberPeclet numberPrandtl numberReynolds numberSherwood numberSchmidt numberStokes number
Definition
a Xl Xx
7]w21 (AAT)
at Itg/3-ATflvl2l(a-tv)aid/3T W2T] IXall Xwll av I apwll T]PJISv l SP-II(T]-W)
Nomenclature:
a: thermal diffusivity (m2/s)g: acceleration due to gravity (m/s2)/: characteristic length (m)p: ressure (N/m )t. time (s)
Indices
D, P: memory and process of polymer respectivelyAT: Temperature difference (K)w: Velocity of flow (m/s)O1: Outside heat transfer coefficient [W/(m2 • K)]/J: Coefficient of volumetric expansion (K" )/J1: Temperature coefficient in the power law of viscosity (KT1)(5S: Mass transfer coefficient (m/s)& Diffusion coefficient (m 2 /s)Tj: Viscosity (Ns /m 2 )A: Thermal conduct ivi ty (Index i refers to the inside value) [ W / ( m K)]v: Kinematic viscosity (m 2 /s)tv: Residence t ime (s)p : Densi ty (kg/m 3)
3.4.1 Physical Meaning of Dimensionless Groups
Biot number: Ratio of thermal resistances in series: (/ / A1) / (1 / oQApplication: heating or cooling of solids by heat transfer through conduction andconvection
Brinkmann number: ratio of heat dissipated (T] w ) to heat conducted (AAT)Application: polymer melt flow
Fourier number: ratio of a characteristic body dimension to an approximate temperaturewave penetration depth for a given time [16]Application: unsteady state heat conduction
Deborah number: ratio of the period of memory of the polymer to the duration ofprocessing [13]. At Deb > 1 the process is determined by the elasticity of the material,whereas at Deb < 1 the viscous behavior of the polymer influences the process remarkably.Grashof number: ratio of the buoyant force g /5 • AT f to factional force (v)Application: heat transfer by free convection
Graetz number: ratio of the time to reach thermal equilibrium perpendicular to theflow direction (I2Ia) to the residence time (tv)Application: heat transfer to fluids in motion
Lewis number: ratio of thermal diffusivity (a) to the diffusion coefficient (S)Application: phenomena with simultaneous heat and mass transfer.
Nusselt number: ratio of the total heat transferred (a • /) to the heat by conduction (X)Application: convective heat transfer.
Pedet number: ratio of heat transfer by convection (pc -w-l) to the heat by conductiona)Application: heat transfer by forced convection.
Nahme or Griffith number: ratio of viscous dissipation (j3T W2J]) to the heat byconduction (X) perpendicular to the direction of flowApplication: heat transfer in melt flow
Prandtl number: ratio of the kinematic viscosity (v) to thermal diffusivity (a)Application: convective heat transfer
Reynolds number: ratio of the inertial force (p w I) to viscous force (T])Application: The Reynolds number serves as a criterium to judge the type of flow. Inpipe flow, when Re is less than 2300 the flow is laminar. The flow is turbulent at Regreater than about 4000. Between 2100 and 4000 the flow may be laminar or turbulentdepending on conditions at the entrance of the tube and on the distance from the entrance[2]Application: fluid flow and heat transfer.
Sherwood number: ratio of the resistance to diffusion (/ / S) to the resistance to masstransfer (l/j8s)Application: mass transfer problems
Schmidt number: ratio of kinematic viscosity (v) to the diffusion coefficient (S)Application: heat and mass transfer problems
Stokes number: ratio of pressure forces (p • Z) to viscous forces (rj • w)Application: pressure flow of viscous media like polymer melts.The use of dimensionless numbers in calculating non Newtonian flow problems isillustrated in Section 4.3.3 with an example.
3.5 Heat Transfer by Convection
Heat transfer by convection, particularly by forced convection, plays an important rolein many polymer processing operations such as in cooling a blown film or a part in aninjection mold, to mention only two examples. A number of expressions can be found inthe literature on heat transfer [3] for calculating the heat transfer coefficient a (seeSection 3.1.6). The general relationship for forced convection has the form
(3.53)
The equation for the turbulent flow in a tube is given by [16]
(3.54)
where
n = 0.4 for heatingn = 0.3 for cooling
The following equation applies to laminar flow in a tube with a constant wall temperature[3]
(3.55)
where
d{ = inside tube diameter/ = tube length
The expression for the laminar flow heat transfer to flat plate is [3]
(3.56)
Equation 3.56 is valid for Pr = 0.6 to 2000 and Re < 105.
The equation for turbulent flow heat transfer to flat plate is given as [3]
(3.57)
Equation 3.57 applies for the conditions:
Pr = 0.6 to 2000 and 5 • 105 < Re < 107.
The properties of the fluids in the equations above are to be found at a mean fluidtemperature.
Example
A flat film is moving in a coating equipment at a velocity of 130 m/min on rolls that are200 mm apart. Calculate the heat transfer coefficient a if the surrounding medium is airat a temperature of 50 0C.
Solution
The properties of air at 50 0C are:
Kinematic viscosity v = 17.86 • 10"6 m2/sThermal conductivity A = 28.22 • 10"3 W/(m • K)Prandtl number Pr = 0.69
The Reynolds number ReL, based on the length L = 200 mm is
Substituting ReL = 24262 and Pr = 0.69 into Equation 3.56 gives
As the fluid is in motion on both sides of the film, the Nusselt number is calculatedaccording to [3]
For turbulent flow Nu111^ follows from Equation 3.57:
The resulting Nusselt number Nu is
Heat transfer coefficient a results from
3.6 Heat Transfer by Radiat ion
Heating by radiation is used in thermoforming processes to heat sheets or films, so thatthe shaping process can take place. Because at temperatures above 300 0C a substantialpart of the thermal radiation consists of wavelengths in the infrared range, heat transferby radiation is also termed as infrared radiation [14]. According to the Stefan-Boltzmannlaw the rate of energy radiated by a black body per unit area es is proportional to theabsolute temperature T to the fourth power (Figure 3.13) [I]:
(3.58)
The Stefan-Boltzmann constant has the value
Equation 3.58 can also be written as
(3.59)
where cs = 5.77 W/(m2 • K4)
The dependence of the black body radiation on the direction (Figure 3.14) [1] is givenby the cosine law of Lambert
(3.60)
The radiation properties of technical surfaces are defined as (Figure 3.15) [I]:
Reflectivity
Absorptivity
Transmissivity
The sum of these fractions must be unity, or
p + a+8 =1
The transmissivity 8 of opaque solids is zero so that
p + a= 1
The reflectivity of gases p is zero and for those gases which emit and absorb radiation
a+8=l
Real bodies emit only a fraction of the radiant energy that is emitted by a black body atthe same temperature. This ratio is defined as the emissivity e of the body,
(3.64)
(3.61)
(3.62)
(3.63)
Figure 3.13Black body radiation [1]
Figure 3.14Lambert's law[1]
Figure 3.15Properties of radiation
At thermal equilibrium according to Kirchhoff s identity
8= a (3.65)
Radiation heat transfer between nonblack surfaces.
The net rate of radiant heat exchange between two infinite parallel plates is given by [15]
(3.66)
where
A = areaC12 = emissivity factor and is defined by
(3.67)
Indices 1 and 2 refer to the two plates.
When T2 is much smaller than T1, the heat flow is approximately
(3.68)
When the heat transfer takes place by radiation and convection, the total heat transfercoefficient can be written as [15]
^total = ^convection ~*~ ^radiation
where
Example
A plastic sheet moving at a speed of 6 m/min is heated by two high-temperature heatingelements. Calculate the power required for heating the sheet from 20 0C to 140 0C:
net enthalpy of the plastic for a temperature difference of 120 0C: Ah = 70 kj/kg
Width of the sheet w =600 mmThickness s = 250 |iDensity of the resin p = 900 kg/m3
Area of the heating element A = 0.0093 m2
Emissivity of the heater £ = 0.9
Solution
Heating power Nn:
Mass flow rate of the plastic m :
As the area of the heating element is small compared to that of the sheet the equationapplies [14]
total area of the heating element Ag = 2 • A so that we have
T= 9.95
100T = 995 K
3.7 Dielectric Heat ing
The dielectric heat loss that occurs in materials of low electrical conductivity when placedin an electric field alternating at high frequency is used in bonding operations, for example,to heat-seal plastic sheets or films.
The power dissipated in the polymer is given by [14]
(3.69)
where
Nn= power (W)/ = frequency of the alternating field (s"1)C = capacitance of the polymer (farads)E = applied voltage (Volt)0 = phase angle
The rate of heat generation in a plastic film can be obtained from Equation 3.69 andgiven as [15]
(3.70)
where
Nn= rate of heat generation (W/m3)£* = dielectric loss factorb = half thickness of the film (\i)
Example
Given:
E = 500 V/ = 10 MHz€* = 0.24b =50 Ji
Calculate the rate of heat generation and the time required to heat the polymer from20 0C to 150 0C.
Substituting the given values in Equation 3.70 gives
The maximum heating rate AT per second is calculated from
For
Finally the heating time is
(3.71)
3.8 Fick's Law of Diffusion
Analogous to Fourier's law of heat conduction (Equation 3.1) and the equation for shearstress in shear flow, the diffusion rate in mass transfer is given by Fick's law. This can bewritten as [16]
(3.72)
where
mA = mass flux per unit timeA - AreaD^B = diffusion coefficient of the constituent A in constituent BcA = mass concentration of component A per unit volumex = distance.
The governing expression for the transient rate of diffusion is [2]
(3.73)
where
t = timex = distance
The desorption of volatile or gaseous components from a molten polymer in an extrudercan be calculated from [17] using Equation 3.73
(3.74)
where
^ 1 = rate of desorption (g/s)Ac = area of desorption (cm2)C0 = initial concentration of the volatile component (g/cm3) in the polymerD = diffusion coefficient (cm2/s)t - time of exposure (s) of the polymer to the surrounding atmosphere
3.8.1 Permeability
Plastics are permeable by gases, vapors and liquids to a certain extent. The dififiisionalcharacteristics of polymers can be described in terms of a quantity known as per-meability.
The mass of the fluid permeating through the polymer at equilibrium conditions is givenby [7]
(3.75)
where
m - mass of the fluid permeating (g)p = permeability [g/(m • s • Pa)]t = time of diffusion (s)A = area of the film or membrane (m2)Pv Pi = Partial pressures on the side 1 and 2 of the film (Pa)s = thickness of the film (mm)
In addition to its dependence on temperature, the permeability is influenced by thedifference in partial pressures of the fluid and thickness of the film. Other factorsinfluencing permeability are the structure of the polymer film, such as crystallinity, andthe type of fluid.
3.8.2 Absorption and Desorption
The process by which the fluid is absorbed or desorbed by a plastic material is time-dependent, governed by its solubility and by the diffusion coefficient [7]. The perioduntil equilibrium value is reached can be very long. Its magnitude can be estimated bythe half-life of the process given by [7]
(3.76)
where
t05 = half life of the processs = thickness of the polymer assumed to be penetrated by one sideD = diffusion coefficient
The value of tQ 5 for moisture in polymethyl methacrylate (PMMA) for
and s = 3 mm
is 17.1 days when the sheet is wetted from one side only [7]. However, the equilibriumabsorption takes much longer, as the absorption rate decreases with saturation.
References
[I] BENDER, E.: Lecture notes, Warme and Stoffiibergang, Univ. Kaiserslautern (1982)
[2] MCCABE, W. L., SMITH, J. C , HARRIOTT, P.: Unit Operations of Chemical Engineering. McGrawHill, New York (1985)
[3] MARTIN, H.: in VDI Warmeatlas, VDI Verlag, Diisseldorf (1984)
[4] WELTY, J. R., WICKS, C. E., WILSON, R. E.: Fundamentals of Momentum, Heat and Mass Transfer,John Wiley, New York (1983)
[5] KREITH, E, BLACK, W. Z.: Basic Heat Transfer, Harper & Row, New York (1980)
[6] THORNE, J. L.: Plastics Process Engineering, Marcel Dekker, New York (1979)
[7] OGORKIEWICZ, R. M.: Thermoplastics - Properties and Design, John Wiley, New York (1974)
[8] WUBKEN, G.: Berechnen von Spritzgiefiwerkzeugen, VDI Verlag, Diisseldorf (1974)
[9] GERSTEN, K.: Einfuhrung in die Stromungsmechanik, Vieweg, Braunschweig (1981)
[ 10] WINTER, H. H.: Extruder als Plastifiziereinheit, VDI Verlag, Diisseldorf (1977)
[II] RAUWENDAAL, C.: Polymer Extrusion, Hanser Publishers, Munich (2001)
[12] KREMER, H.: Grundlagen der Feuerungstechnik, Engler-Bunte-Institut, Univ. Karlsruhe (1964)
[13] COGSWELL, F. N.: Polymer Melt Rheology, George Godwin, London (1981)
[ 14] BERNHARDT, E. C.: Processing of Thermoplastic Materials, Reinhold, New York (1959)
[15] MCKELVEY, J. M.: Polymer Processing, John Wiley, New York (1962)
[16] HOLMAN, J. P.: Heat Transfer, McGraw Hill, New York (1980)
[17] SECOR, R. M.: Polym. Eng. ScL 26 (1986) p. 647
4 D e s i g n i n g P l a s t i c s P a r t s
The deformational behavior of polymeric materials depends mainly on the type andmagnitude of loading, time of application of the load, and temperature. The deformationis related to these factors in a complex manner, so that the mathematical treatment ofdeformation requires a great computational effort [I]. However, in recent times computa-tional procedures for designing plastic parts have been developed using stress-strain data,which were carefully measured by employing computer-aided testing of polymers [2].
4.1 S t r e n g t h o f P o l y m e r s
The basic equation for calculating the design stress of a part under load is given by [ 1 ]
(4.1)
where
K = material strength as a mechanical propertyav = maximum stress occurring in the part°zui ~ allowable stressS = factor of safetyA = material reduction factor
The relation between allowable stress and the polymer-dependent reduction factors canbe written as [1]
(4.2)
The factor A 0 considers the influence of temperature on the strength of the material andcan be calculated from [1]
(4.3)
where 0 = temperature. The limits of applicability of Equation 4.3 are 20 < 0 < 100 0C.
The value k based on the reference temperature of 20 0C is given for the following materialsas[ l ]
PA66 =0.0112PA6 = 0.0125PBT = 0.0095
GR-PA and GR-PBT =0 .0071P O M = 0.0082ABS =0 .0117
The other reduction factors in Equation 4.2 consider the following effects:
The factor Ast represents the effect of the t ime of static loading and can have followingvalues depending on t ime [ I ] :
time hours weeks months years
Ast 1.3 1.6 1.7 2
The factor Ad y n takes the effect of dynamic loading into account and lies in the range of1.3 to 1.6.
The factor AA, considers the influence of aging and has to be determined experimentally.
The reduction of strength caused by the absorption of moisture by the plastic can beestimated from the factor A w . For unreinforced polyamides A w is roughly [ 1 ]
(4.4)
with /ranging from 0 < / < 3 where/= weight percentage of moisture. The value of Aw is3.4 when/is greater than 3.
4.2 Part Failure
Usually stresses resulting from loading of the part are multiaxial. Because measuredmaterial properties do not exist for combined stresses, the multiaxial state has to bereduced to an uniaxial state by applying the principle of equivalence. According to HUBER,
VON MISES and HENKY [1] the governing equation for the equivalent stress is
(4.5)
where CT1, G1 and (T3 are normal stresses. The equivalent strain £ is defined by [3]
(4.6)
Materials, whose compressive stress is higher than the tensile stress, can be better describedby the conical or parabolic criterion [I]. The equivalent stress CT , according to theconical criterion, is given as [ 1 ]
where m is the ratio of compressive stress to tensile stress.
Example
Figure 4.1 [1] shows a press fit assembly consisting of a metal shaft and a hub made ofPOM. The joint strength can be determined as follows:
For the numerical values rJrY = 1.6 and p = 22 N/mm2 the equivalent stress is to becalculated.
The tangential stress Gx is given by
Substituing the values above
The radial compressive stress G1 is
(4.9)
Figure 4.1 Stress analysis in a press fit hub
(N]
The parabolic failure criterion is defined by
(4.8)
(4.7)
Substituting Gx = 50.2 N/mm2, G2 = -22 N/mm2 and G3 = 0 in Equation 4.5 gives
The equivalent stress Cv y according to Equation 4.7 for the conical failure criterion, isobtained from
wi thm= 1.4 for POM.
The yield point of POM is around 58 N/mm2. Thus, the assumed joint strength is toohigh. In the case of deformation of the part by shear, the shear stress is given by [I]
T = 0.5 O (4.10)
4.3 T ime-Dependent Deformat ional Behavior
4.3.1 Short-Term Stress-Strain Behavior
As mentioned in Section 1.4, polymers are viscoelastic materials and their deformationalbehavior is nonlinear. A typical stress-strain curve of POM under short-term loading isshown in Figure 4.2. Curves of this type can be expressed by a fifth degree polynomial ofthe form [4]
(4.11)
where PK0 ... PK5 are polynomial coefficients dependent on the resin at a given tempera-ture.
Figure 4.2 Stress-strain diagram for POMStrain £
%
Stre
ss 6
N/mm2
The secant modulus (Figure 4.3) is given by
(4.12)
Setting PK0 = 0 it follows from Equation 4.11
(4.13)
4.3.2 Long-Term Stress-Strain Behavior
The dimensioning of load bearing plastic components requires knowledge of stress-straindata obtained under long-term loading at different temperatures. Retardation experimentsprovide data on time-dependent strain in the form of creep plots, see Figure 4.4a. InFigure 4.4b the stress is given as a function of time for different values of strain.Isochronous stress-strain-time curves are illustrated in Figure 4.4c.
The critical strain method according to MENGES [10] provides a useful criterion fordesigning plastic parts. The experiments of MENGES and TAPROGGE [10] show that safedesign is possible when the critical strain is taken as the allowable deformation. Thecorresponding tensile stress can be obtained from the isochronous stress-strain diagram.
The expression for calculating the time-dependent strain according to FINDLEY [8] is givenas
(4.14)
The power function of FINDLEY [2] is written as
(4.15)
The function for the coefficient m is a fifth degree polynomial and that of n is a straightline. With the Findley power function the long-term behavior of plastics up to 105 hourscan be described on the basis of measurements covering shorter periods of approx. 103
hours [2].
Stre
ss 6
Strain £Figure 4.3 Secant modulus [4]
Figure 4.4 Long-term stress-strain behavior [7]
Example [9]
The minimum depth of the simple beam made of SAN shown in Figure 4.5 is to bedetermined for the following conditions:
The beam should support a mid-span load of 11.13 N for 5 years without fracture andwithout causing a deflection exceeding 2.54 mm.
Stra
in S
Stre
ss 6
Stre
ss 6
Time /
Time t Strain £
Figure 4.5 Beam under midspan load [9]
Solution
The maximum stress is given by
(4.16)
a
cb
where
P = load (N)Lybyd = dimensions in (mm) as shown in Figure 4.5
The creep modulus Ec is calculated from
where / is deflection in mm. The maximum stress from Figure 4.6 after a period of 5 years(= 43800 h) is
CJmax 23.44 N/mm2
(4.17)
Initia
l app
lied
stres
s
Cree
p mo
dulus
Time at ruptureFigure 4.6 Creep curve for SAN [9]
Time tFigure 4.7 Creep modulus for SAN [9]
mm2
h
h
JLmm2
Working stress <7W with an assumed safety factor S = 0.5:
Creep modulus Ec at O < <TW and a period of 5 years from Figure 4.7
Creep modulus Ec with a safety factor S = 0.75:
Ec = 2413 • 0.75 = 1809.75 N/mm2
The depth of the beam results from Equation 4.16
The deflection is calculated from Equation 4.17
/ i s smaller than 2.54 mm.
References
[1] ERHARD, G.: Berechnen von Kunststoff-Formteilen VDI-Verlag, Diisseldorf (1986)
[2] HAHN, H.: Berechnen von Kunststoff-Formteilen, VDI-Verlag, Diisseldorf (1986)
[3] OGORKIEWICZ, R. M.: Thermoplastics Properties and Design, John Wiley, New York (1973)
[4] AUMER, B.: Berechnen von Kunststoff-Formteilen, VDI-Verlag, Diisseldorf (1986)
[5] RAO, N.: Designing Machines and Dies for Polymer Processing, Hanser Publishers, Munich(1981)
[6] Werkstoffblatter, BASF Kunststoffe, BASF, Ludwigshafen
[7] BERGMANN, W.: Werkstofftechnik Teil 1, Hanser Publishers, Munich (1984)
[8] FINDLEY, W. N.: ASTM Symposium on Plastics (1944) p. 18
[9] Design Guide, Modern Plastics Encyclopedia (1978-1979)
[10] MENGES, G., TAPROGGE, R.: Kunststoff-Konstruktionen. VDI-Verlag Dusseldorf (1974)
5 F o r m u l a s f o r D e s i g n i n g E x t r u s i o n
a n d I n j e c t i o n M o l d i n g E q u i p m e n t
5.1 E x t r u s i o n Dies
The design of extrusion dies is based on the principles of rheology, thermodynamics,and heat transfer, which have been dealt with in Chapters 2 to 4. The strength of thematerial is the determining factor in the mechanical design of dies. The major quantitiesto be calculated are pressure, shear rate, and residence time as functions of the flow pathof the melt in the die. The pressure drop is required to predict the performance of thescrew. Information on shear rates in the die is important to determine whether the meltflows within the range of permissible shear rates. Overheating of the melt can be avoidedwhen the residence time of the melt in the die is known, which also provides an indicationof the uniformity of the melt flow.
5.1.1 Calculation of Pressure Drop
The relation between volume flow rate and pressure drop of the melt in a die can beexpressed in the general form as [2]
(5.1)
where
Q = volume flow rateG = die constantAp = pressure differenceK = factor of proportionality in Equation 1.26n = power law exponent Equation 1.30
It follows from Equation 5.1
(5.2)
5.1.1.1 Effect of Die Geometry on Pressure Drop
The die constant G depends on the geometry of the die. The most common geometriesare circle, slit and annulus cross-sections. G for these shapes is given by the followingrelationships [2].
where
£ = RadiusL = Length of flow channel
(5.4)
Wfor — > 20
Hwhere H is the height of the slit and W is the width.
WFor — < 20, Gslit has to be multiplied by the correction factor Fp given in Figure 5.1
H
The factor F can be expressed as
(5.5)
The die constant G3J1n 118 is calculated from
(5.6)
and(5.7)
where R0 is the outer radius and JR1 is the inner radius. Gannulus then follows fromEquation 5.4
Corre
ction
fac
tor f
p
Channel depth to width ratio H/W
Figure 5.1 Correction factor Fp as a function of H/W [12]
WH
(5.3)
for values of the ratio n (R0 + R1) I (R0 - JR1) > 37
For smaller values of this ratio, Ga1111111118 has to be multiplied by the factor Pp given inFigure 5.1. The height H and width W are obtained in this case from Equation 5.6 andEquation 5.7.
5.1.1.2 Shear Rate in Die Channels
The shear rate for the channels treated above can be computed from [3]
(5.9)
(5.10)
(5.11)
The shear rate for an equilateral triangle is given by [4]
(5.12)
where d is the half length of a side of the triangle.
The relation for a quadratic cross-section is [4]
(5.13)
where a is the length of a side of the square.
In the case of channels with varying cross-sections along the die length, for example,convergent or divergent channels, the channel is divided into a number of sufficientlysmall increments and the average dimensions of each increment are used in the equationsgiven above [3].
5.1.1.3 General Relation for Pressure Drop in Any Given Channel Geometry
By means of the substitute radius defined by SCHENKEL [5] the pressure drop in cross-sections other than the ones treated in the preceding sections can be calculated. Thesubstitute radius is expressed by [5]
(5.8)
where
Rrh= substitute radiusA - cross-sectional areaB = circumference
5.1.1.4 Examples
The geometrical forms of the dies used in the following examples are illustrated inFigure 5.2.
Example 1
It is required to calculate the pressure drop Ap of a LDPE melt at 200 0C flowing througha round channel, 100 mm long and 25 mm diameter, at a mass flow rate of m = 10 g/s .
The constants of viscosity in the Equation 1.36 for the given LDPE are
A0 = 4.2968A1 = -3.4709 • 10"1
A2 =-1.1008- 10"1
A3 = 1.4812 • 10"2
A4 =-1.1150-HT3
(5.14)
Figure 5.2 Flow channel shapes in extrusion dies
melt density p m = 0.7 g/cm3
Solution
Volume flow rate Q = — = — = 14.29 cm3/s = 1.429 • 10~5 m3/sAn 0.7
Shear rate f^ from Equation 5.9:
Shift factor aT from Equation 1.34:
By Equation 1.37, the power law exponent n is
Substituting the constants A1 ... A4 results in
n = 1.832
Viscosity 7]a from Equation 1.36
With aT = 0.374, yz = 9.316 and the constants A0 ... A4 we get
Shear stress T from Equation 1.22
Factor of proportionality K from Equation 1.26:
Die constant Gcirde from Equation 5.3:
Pressure drop from Equation 5.2:
Example 2
Melt flow through a slit of width W = 75 mm, height H = 1 mm, and length L = 100 mm.
The resin is LDPE with the same viscosity constants as in Example 1. The mass flow rateand the melt temperature have the same values, m = 10 g/s and T = 200 0C. The pressuredrop Ap is to be calculated.
Solution
Volume flow rate
Shear rate from Equation 5.10:
Shift factor aT from Equation 1.34:
power law exponent n from Equation 1.37:
Viscosity 7]a from Equation 1.36:
Shear stress T from Equation 1.22:
Proportionality factor K from Equation 1.26:
Correction factor Fp
As the ratio W/H is greater than 20, the die constant which can be calculated fromEquation 5.4 need not be corrected.
and finally the pressure drop Ap from Equation 5.2
Example 3
Melt flow through a slit with width W = 25 mm, height H= 5 mm, and length L = 100 mm.
The resin is LDPE with the same viscosity constants as in Example 1. The mass flow ratem = 10 g/s and the melt temperature T = 200 0C. The pressure drop Ap is to be calculated.
Solution
Volume flow rate
Shear rate ya from Equation 5.10:
Shift factor ar from Equation 1.34:
Power law exponent n from Equation 1.37:
Viscosity 7]a from Equation 1.36:
Shear stress T from Equation 1.22:
Proportionality factor K from Equation 1.26:
Correction factor Fp:
As the ratio W/H = 5, which is less than 20, the die constant Gslit has to be corrected.Fp from Equation 5.5:
Pressure drop Ap from Equation 5.2:
Example 4
Melt flow through an annulus with an outside radius R0 = 40 mm, an inside radiusR1 = 39 mm, and of length L = 100 mm.
The resin is LDPE with the same viscosity constants as in Example 1. The processparameters, mass flow rate, and melt temperature remain the same.
Solution
Volume flow rate
Shear rate y^ from Equation 5.11:
Shift factor aT from Equation 1.34:
Power law exponent n from Equation 1.37:
n = 2.907
Viscosity 7]a from Equation 1.36:
?7a = 579.43 Pa • s
Shear stress T from Equation 1.22:
T= 200173.6 N/m2
Factor of proportionality K from Equation 1.26:
K= 1.3410 -10"13
Correction factor Fp
As the ratio — = 248.19 is greater than 37, no correction is necessary.
Gannuius from Equation 5.8:
Pressure drop Ap from Equation 5.2
Example 5
Melt flow through a quadratic cross section with the length of a side a = 2.62 mm. Thechannel length L = 50 mm. The resin is LDPE with the following constants for the powerlaw relation in Equation 1.32:
Following conditions are given:
mass flow ratemelt temperaturemelt density
The pressure drop Ap is to be calculated.
Solution
Three methods of calculation will be presented to find the pressure drop in this example.
Method a
With this method, the melt viscosity is calculated according to the power law. Other thanthat, the method of calculation is the same as in the foregoing examples.
Volume flow rate
Shear rate
For a square with W=H the shear rate yz is
Power law exponent n:
Viscosity rja from Equation 1.32:
Shear stress T from Equation 1.22:
T= 40434.88 N/m2
Proportionality factor K from Equation 1.26:
K= 4.568 -1(T14
Correction factor Fp
WAs — = 1 is less than 20, the correction factor is obtained from Equation 5.5
H
fp = 1.008 - 0.7474 • 1 + 0.1638 • I2 = 0.4244
Die constant Gslit from Equation 5.4:
Gslit =4.22 • 10"5
G8Ut corrected = 0-4244 • 4.22-10"5 = 1.791 • 10-5
Pressure drop Ap from Equation 5.2:
Method b
The shear rate ya is calculated from Equation 5.13
Viscosity ?]a from Equation 1.32:
77a = 24205.54 • 5.67403286"1 = 7546.64 Pa • s
Shear stress T from Equation 1.22:
T= 42819.6 N/m2
Power law exponent n from Equation 1.28:
Proportionality factor K from Equation 1.26:
K= 4.568 -10"14
The pressure drop Ap is found from
(5.15)
with the die constant Gsquare
(5.16)
In Equation 5.15
Finally Apsquare from Equation 5.2:
The above relationship for shear rate developed by RAMSTEINER [4] leads to almost thesame result as obtained by Method a.
Method c
In this method, a substitute radius is calculated from Equation 5.14; the pressure drop isthen calculated using the same procedure as in the case of a round channel (Example 1):
Substitute radius .Rrh:
Shear rate % from Equation 5.13:
Viscosity ?]a from Equation 1.32:
7]a = 24205.54 • 7.1830'3216"1 = 6441.56 Pa • s
Shear stress T from Equation 1.22:
T = 46269.73 N/m2
Factor of proportionality from Equation 1.26:
K = 4.568- 10"14
circle fr°m Equation 5.3:
Pressure drop from Equation 5.2:
This result shows that the relationship, Equation 5.14 [5], is sufficiently accurate forpractical purposes. This equation is particularly useful for dimensioning channels, whosegeometry differs from the common shape, that is, circle, slit or annulus. The procedureof calculation for an equilateral triangle is shown in the following example:
Example 6
Melt flow through an equilateral triangular channel of length L = 50 mm. The side of thetriangle 2 d = 4.06 mm. Other conditions remain the same as in Example 5.
Solution
Substitute radius Rrh from Equation 5.14 with
n = 3.043
RTh= 1.274 mm
Shear rate / a from Equation 5.9:
Viscosity 7]a from Equation 1.32:
77a = 24205.54 • 8.80 '328" = 5620.68 Pa • s
Shear stress T from Equation 1.22:
T= 49462 N/m2
Factor of proportionality from Equation 1.26:
K= 4.568-10"14
Gcircle from Equation 5.3:
Pressure drop Ap from Equation 5.2:
Using the relation developed by RAMSTEINER [4] on the basis of rheological measurementon triangular channels, Example 6 is calculated as follows for the purpose of comparingboth methods:
Shear rate from Equation 5.12:
Viscosity 7]a from Equation 1.32:
7]a = 24205.54 • 5.6920'3286"1 = 7530.61 Pa • s
Shear stress T from Equation 1.22:
T = 42864.2 N/m2
Factor of proportionality from Equation 1.26:
K= 4.568 -10"14
This result differs little from the one obtained by using the concept of substitute radius.Therefore this concept of SCHENKEL [5] is suitable for use in practice.
5.1.1.5 Temperature Rise and Residence Time
The adiabatic temperature increase of the melt can be calculated from
(5.18)
where
AT = temperature rise (K)Ap = pressure difference (bar)p m = melt density (g/cm3)cpm = specific heat of the melt kj/(kg • K)
The residence time T of the melt in the die of length L can be expressed as
(5.19)
u = average velocity of the melt
Equation 5.19 for a tube can be written as
(5.20)
R = tube radiusya = shear rate according to Equation 5.9
Die constant Gtriangle:
(5.17)
Pressure drop Ap from Equation 5.2:
The relation of a slit is
(5.21)
H = height of slitya = shear rate according to Equation 5.10
5.1.1.6 Adapting Die Design to Avoid Melt Fracture
Melt fracture can be defined as an instability of the melt flow leading to surface or volumedistortions of the extrudate. Surface distortions [34] are usually created from instabilitiesnear the die exit, while volume distortions [34] originate from the vortex formation atthe die entrance. Melt fracture caused by these phenomena limits the production of articlesmanufactured by extrusion processes. The use of processing additives to increase theoutput has been dealt with in a number of publications given in [35]. However, processingaids are not desirable in applications such as pelletizing and blow molding. Therefore,the effect of die geometry on the onset of melt fracture was examined.
The onset of melt fracture with increasing die pressure is shown for LDPE and HDPE inFigure 5.3 [38]. As can be seen, the distortions appear differently depending on the resin.The volume flow rate is plotted in Figure 5.4 [39] first as a function of wall shear stressand then as a function of pressure drop in the capillary for LDPE and HDPE. The suddenincrease in slope is evident for LDPE only when the flow rate is plotted against pressure,whereas in the case of HDPE it is the opposite. In addition, for HDPE the occurrence ofmelt fracture depends on the ratio of length L to diameter D of the capillary. The effectof temperature on the onset of melt fracture is shown in Figure 5.5 [36]. With increasingtemperature the onset of instability shifts to higher shear rates. This behavior is used inpractice to increase the output. However, exceeding the optimum processing temperaturecan lead to a decrease in the quality of the product in many processing operations. Fromthese considerations it can be seen that designing a die by taking the resin behavior intoaccount is the easiest method to obtain quality products at high throughputs.
Design procedure
Using the formulas given in this book and in reference [33], the following design procedurehas been developed to suit the die dimensions to the melt flow properties of the resin tobe processed with the die.
STEP 1: Calculation of the shear rate in the die channelSTEP 2: Expressing the measured viscosity plots by a rheological modelSTEP 3: Calculation of the power law exponentSTEP 4: Calculation of the shear viscosity at the shear rate in Step 1STEP 5: Calculation of the wall shear stressSTEP 6: Calculation of the factor of proportionalitySTEP 7: Calculation of die constant
N/mm2
LDPE
HDPE
Figure 5.3 lrregularties of the extrudate observed at increasing extrusion pressure with LDPE andHDPE [38]
Figure 5.4 Volume rate vs. wall shear stress and vs. pressure drop in capillary for LDPE and HDPE [39]
LDPE HDPE
In ApInAp
InQInQ
In <7W In (T0,
InQInQ
r Shear stress (N/m2)Figure 5.5 Effect of temperature on the melt fracture (region 2) for HDPE
STEP 8: Calculation of pressure drop in the die channel andSTEP 9: Calculation of the residence time of the melt in the channel
Applications
Based on the design procedure outlined above, computer programs have been developedfor designing dies for various processes. The principles of the design methods areillustrated below for each process by means of the results of the simulation performedon the dies concerned. The designing principle consists basically of calculating the shearrate, pressure drop, and residence time of the melt during its flow in the die and keepingthese values below the limits at which melt fracture can occur. This is achieved by changingthe die dimensions in the respective zones of the die, in which the calculated values mayexceed the limits set by the resin rheology.
y Sh
ear r
ate
(sec
1)
HDPE
3 ,
2
Figure 5.6 Simulation results for a pelletizer die
a) Pelletizer Dies
The aim here is to design a die for a given throughput or to calculate the maximumthroughput possible without melt fracture for a given die. These targets can be achievedby performing simulations on dies of different tube diameters, flow rates, and melttemperatures. Figure 5.6 shows the results of one such simulation.
b) Blow Molding Dies
Figure 5.7 shows a blow molding parison and the surface distortion that occurs at a specificshear rate depending on the resin. In order to obtain a smooth product surface, the diecontour has been changed in such a way that the shear rate lies in an appropriate range(Figure 5.8). In addition, the redesigned die creates lower extrusion pressures, as can beseen from Figure 5.8 [36].
c) Blown Film Dies
Following the procedure outlined above and using the relationships for the differentshapes of the die channels concerned, a blown film spider die was simulated (Figure 5.9).On the basis of these results it can be determined whether these values exceed the boundaryconditions at which melt fracture occurs. By repeating the simulations, the die contourcan be changed to such an extent that shear rate, shear stress, and pressure drop arewithin a range, in which melt fracture will not occur. Figure 5.10 and 5.11 show theshear rate and the residence time of the melt along the flow path [37].
The results of simulation of a spiral die are presented in Figure 5.12 as an example. As inthe former case, the die gap and the geometry of the spiral channel can be optimized forthe resin used on the basis of shear rate and pressure drop.
Flow rate: 350 kg/hTemperature: 280 0C LDPE
Die length (mm)
g: Shear ratet Residence time
P(bar)
t(1/s)
t
9
1414.7/S0.0005654 s
Figure 5.7 Surface distortion on a parison used in blow molding
Old die
New die
New dieOld die
Flow length
Pressure
K
Figure 5.8 Die contour used for obtaining a smooth parison surface
Pres
sure
dro
p Ap
(bar
)Sh
ear r
ate
(s 1
)
Length of flow path I (mm)
Figure 5.9 Calculated pressure drop in a spider die with different die gaps used for blown film
LDPE
m = 40 kg/hTM =160 0C
LDPETM =160°ChT =2 mm
Figure 5.10 Shear rate along spider die
Length of flow path I (mm)
Resid
ence
tim
e t (
s)LDPE
m = 40 kg/hTM =160 0C/7r =2 mm
Length of flow path I (mm)
Figure 5.11 Residence time t of the melt as a function of the flow path I
Spiral gap(mm)
37.123 bar54.88/s
p: Total pressure dropga: Shear rate in the gap
P(bar)
fa(1/s)
Shear rate in the gapSpiral gap
Pressure dropinletoutlet
Die length (mm)
Figure 5.12 Results of simulation of a spiral die used for LLDPE blown film
Length of the manifold (mm)
Figure 5.13 Manifold radius as a function of the distance along the length of the manifold
d) Extrusion Coating Dies
Taking the resin behavior and the process conditions into account, the flat dies used inextrusion coating can be designed following similar rules as outlined above. Figure 5.13shows the manifold radius required to attain uniform melt flow out of the die exit as afunction of the manifold length [37].
5.1.1.7 Designing Screen Packs for Extruders
Screen packs are used in polymer processing extruders to remove undesired participatematter from the melt and are placed behind the breaker plate at the end of an extrusionscrew (Figure 5.16). Another important reason to implement screen packs is theirassistance in better back mixing of the melt in an extruder channel, which results fromthe higher resistance offered by the screen to the melt flow. Better back mixing in turnimproves the melt homogenity. In addition, screen packs may also be used to attain highermelt temperatures to enable better plastication of the resin. Owing to the intimaterelationship between melt pressure and extruder throughput it is important to be able topredict the pressure drop in the screen packs as accurately as possible.
Design Procedure
The volume flow rate q through a hole for a square screen opening (Figure 5.14) is givenby [42]
Sketch
Manifoldradius (mm)
Manifold inlet radius:Pressure drop:Manifold angle:
24.84 mm12.23 bar60.34°
Figure 5.15 Screen pack with screens of varied mesh size
The shear rate of the melt flow for a square opening is calculated from
By means of these equations and the design procedure outlined in Section 4.1, followingexamples were calculated and the results are shown in Figure 5.17 to Figure 5.20.
Figure 5.14 Mesh of a wire-gauze screen
meltDs
mn
25.4 mm(1 inch)
do
d\
Table 5.1 Dimensions of Square Screens [41 ]
Mesh size
42100200325
Sieve openingmm
0.3540.1490.0740.044
Nominal wire diametermm
0.2470.1100.0530.030
FlangeDie
Breaker piateScreen pack Meit pressure
Melt temperature
Figure 5.16 Position of screen pack in an extruder [43]
Pres
sure
dro
p in
scre
en(b
ar)
Pres
sure
dro
p in
scre
en
HDPE LDPE LLDPE PET
Type of Polymer
Figure 5.17 Effect of polymer type on pressure drop Ap in the screen pack
HDPEExtruder dia Db = 114.3 mmMelt temperature T= 232 0CMesh size Pnn = 42
Extruder throughput (kg/h)
Figure 5.18 Extruder throughput
Per cent blocked screen area (%)
Figure 5.20 Effect of reduced screen area on the pressure drop in the screen
5.2 Extrusion Screws
In this chapter, formulas for the quantities often required when dimensioning extrusionscrews are illustrated by specific examples.
5.2.1 Solids Conveying
Under the assumptions that:
(a) the polymer moves through the screw channel as a plug,(b) there is no friction between the solid plastic and the screw, and(c) there is no pressure rise,
Pres
sure
dro
p in
scr
een
Pres
sure
dro
p in
scre
en
Mesh sizeFigure 5.19 Effect of the mesh size on the pressure drop in the screen
HDPEExtruder throughput = 454 kg/hMelt temperature T= 232 0CExtruder dia Dt = 114.3 mm
HDPEExtruder throughput = 454 kg/hMesh size nh = 42Extruder dia D0 = 114.3 mm
the maximum flow rate (Qs )max (see Figure 5.21 and Figure 5.22) can be calculated from[6]
(5.22)
(5.23)
(5.24)
The actual flow rate Qs is given by [6]
The conveying efficiency rjF can be expressed as
Figure 5.21 Screw zone of a single screw extruder [7]
Figure 5.22 Movement of solids in a screw channel after TADMOR [6]
In practice, this efficiency is also defined as
(5.25)
where
Gs = mass flow rateN = screw speedV8 = volume of the screw channelpos = bulk density
Example
The geometry of the feed zone of a screw, Figure 5.22, is given by the following data [6]
barrel diameter Dh = 50.57 mmscrew lead s = 50.57 mmnumber of flights V = 1root diameter of the screw Ds = 34.92 mmflight width wFLT = 5.057 mmdepth of the feed zone H = 7.823 mm
The maximum specific flow rate and the actual flow rate are to be calculated.
Solution
Helix angle 0:
Width of the screw channel W:
Maximum specific flow rate from Equation 5.22:
Taking the bulk density pos = 0.475 g/cm3 into account, the specific mass flow rate becomes
The feed angle 0 is required to calculate the actual flow rate. With the assumptions alreadymade and assuming equal friction coefficients on screw/s and barrel^,, the approximatefeed angle may be calculated from [6]
(5.26)
(5.27)
where
With/S =fh - 0.25 and the average diameter
D 3 492With K = 0.522 and —•*- = — = 0.6906 we obtain from Equation 5.26
Db 5.057
Inserting 0 = 15.8° into Equation 5.23
gives
The actual specific mass flow rate using the bulk density pos = 0.475 g/cm3 is therefore
The conveying/ efficiency T]F is
5.2.2 Melt Conveying
Starting from the parallel plate model and correcting it by means of appropriate correctionfactors [7], the throughput of melt in an extruder can be calculated. Although the followingequation for the output applies to an isothermal quasi-Newtonian fluid, it was found tobe useful for many practical applications [3].
For a given geometry of the melt zone (Figure 5.21), the output of a melt extruder orthat of a melt pumping zone of a plasticating extruder can be determined as follows[3,7]
Helix angle </K
(5.28)
(5.29)
(5.30)
(5.31)
(5.32)
(5.33)
(5.34)
Volume flow rate of pressure flow Qp (m3/s):
Mass flow rate rap (kg/h):
Drag flow Qd (m3/s):
Mass flow rate md (kg/h):
The leakage flow through the screw clearance is found from the ratios
and
The extruder output m is finally calculated from
The shear rate required for determining the viscosity ?]a at the given melt temperature Tis obtained from
(5.36)
Symbols and units used in the formulas above:
Db: Barrel diameter mmH: Channel depth mme: Flight width mms: Screw lead mm& Flight clearance mmL: Length of melt zone mmv: Number of flights -Ap: Pressure difference across the melt zone barYi: Shear rate s"1
Qp > Qd: Volume flow rate of pressure flow and drag flow, respectively m3/sthp,md: Mass flow rate of pressure and drag flow, respectively kg/sth: Extruder ou tpu t kg/hTja: Melt viscosity Pa • sad: Ratio of pressure flow to drag flow -T: Melt temperature 0CN: Screw speed min"1
Example
For the following conditions the extruder output is to be determined:
Resin: LDPE with the same constants of viscosity as in Example 1 in Section 4.1.1.
Process parameters:
Screw speed N - 80 min"1 ( rpm)Melt temperature T = 2 0 0 0 CMelt pressure Ap = 300 bar
Geometry of the metering zone:
Dh = 60 m m ; H= 3 m m ; e = 6 m m ; s = 60 m m ; <5pLT = 0.1 m m ; L = 600 m m ; V = I
Solution
fa = 83.8 s"1 Equation 5.36ar = 0.374 Equation 1.347]a = 1406.34 Pa • s Equation 1.360 =17 .66° Equation 5.28m p = -3.146 kg/h Equation 5.29 and Equation 5.30
md = 46.42 kg/h Equation 5.31 and Equation 5.32m = 41.8 kg/h Equation 5.33, Equation 5.34 and Equation 5.35
Leakage flow W1 = rad + mp - m = 1.474 kg/h
5.2.2.1 Correction Factors
To correct the infinite parallel plate model for the flight edge effects, following factors areto be used along with the equations given above:
the shape factor for the drag flow Fd can be obtained from [8] with sufficient accuracy
(5.37)
and the factor for the pressure flow Fp
(5.38)
The expressions for the corrected drag flow and pressure flow would be
The correction factor for the screw power, which is treated in the next section, can bedetermined from [9]
(5.39)
Equation 5.39 is valid in the range 0 < HIW < 2. For the range of commonly occurringH/W-ratios in extruder screws, the flight edge effect accounts for only less than 5% andcan therefore be neglected [8]. The influence of screw curvature is also small so that Fx
can be taken as 1.
Although the above mentioned factors are valid only for Newtonian fluids, their use forpolymer melt flow is justified.
5.2.2.2 Screw Power
The screw power consists of the power dissipated as viscous heat in the channel andflight clearance and the power required to raise the pressure of the melt. Therefore, thetotal power Z N for a melt filled zone [10] is
with
and
where
Zc = power dissipated in the screw channelZFLT = power dissipated in the flight clearanceZAp = power required to raise the pressure of the melt
The power dissipated in the screw channel Zc is given by [10]
(5.41)
The power dissipated in the flight clearance can be calculated from [10]
(5.42)
The power required to raise the pressure of the melt ZAp can be written as
(5.43)
The flight diameter DFLT is obtained from
(5.44)
and the channel width W
(5.45)
The symbols and units used in the equations above are given in the following example:
Example
For the following conditions the screw power is to be determined:
Resin: LDPE with the constants of viscosity as in Example 1 of Section 5.1.1.4
Operating conditions:
screw speed N = 80 rpmmelt temperature T =200 0Cdie pressure Ap = 300 bar
Geometry of the melt zone or metering zone:
D = 60 mm; H — 3 mm; e — 6 mm; 5 = 60 mm; 5pLT = 0.1 mm; AL = 600 mm; V = I
(5.40)
Solution
Power Zc in the screw channel:
DFLT = 59.8 mm from Equation 5.44
Shear rate in the screw channel fc:
yc = 83.8 s"1 from Equation 5.36
aT = 0.374 from Equation 1.34
Viscosity of the melt in the screw channel r\c
ric = 1406.34 Pa • s from Equation 1.36
Channel width W:
W= 51.46 mm from Equation 5.45
Number of flights v:
V= 1
Length of the melt zone AL:
AL = 600 mm
Faktor Fx:
TJ O
Fx = 1 for — = = 0.058 from Equation 5.39W 51.46
Helix angle (fr.
(/) = 17.66°; sin0 = 0.303 from Equation 5.28
Power in the screw channel Zc from Equation 5.41:
Power in the flight clearance ZFLT:
Flight width wFLT (Figure 5.22):
WFLT ~ e c o s 0 = 6 ' cos 17.66° = 5.7 mm
Shear rate in the flight clearance ^FLT:
Shift factor aT:
aT = 0.374 at T= 200 0C from Equation 1.34
Viscosity in the flight clearance rjFLT:
%LT ~ 2 1 9 - 7 P a ' s fr°m Equation 1.36
Length of the melt zone AL:
AL = 600 mm
ZFLT from Equation 5.42:
Power to raise the melt pressure ZAp
Pressure flow Q p :
Qp from the Example in Section 4.2.2
Die pressure Ap:
Ap= 300 bar
Z^p from Equation 5.43:
Z^ = 100 • 1.249 • 10^6 • 300 = 0.0375 kW
Hence the power ZAp is negligible in comparison with the sum Zc + ZFLT.
5.2.2.3 Heat Transfer between the Melt and the Barrel
To estimate the power required to heat the barrel or to calculate the heat lost from themelt, the heat transfer coefficient of the melt at the barrel wall is needed. This can beestimated from [11]
(5.46)
where the thermal diffiisivity a
(5.47)
and the parameter j3
(5.48)
Indices:
m: meltf: melt filmb: barrel
Example with symbols and units
Thermal conductivity Am = 0.174 W/(m • K)Specific heat cpm= 2 kj/(kg • K)Melt density pm = 0.7 g/cm3
Thermal diffusivity a from Equation 5.47:
a=1.243-10~7m2/s
Flight clearance 5pLT =0.1 mmScrew speed N = 80 rpm
Parameter /J from Equation 5.48:
P= 0.027
For Tf = 137.74 0C, Tm = 110 0C and Th = 150 0C
asz from Equation 5.46:
5.2.2.4 Melt Temperature
The exact calculation of melt or stock temperature can be done only on an iterative basisas shown in the computer program given in [9]. The following relationships and thenumerical example illustrate the basis of calculating the stock temperature. The resultobtained can only be an estimate of the real value, as it lacks the accuracy obtained bymore exact iterative procedures.
Temperature rise AT:
(5.49)
Heat through the barrel or heat lost from the melt:
(5.50)
Example for calculating NH with symbols and units
as = 315.5 W/(m2 • K); DFLT = 59 mm; AL = 600 mm; Th = 150 0C; cpm = 2 kj/(kg • K)
Stock temperature at the inlet of the screw increment considered:
T1n = 200 0C
Nn from Equation 5.50:
315.5 -n -59.8 -600 -50 , ft^1TAT,iNH = = -1.86 kW (heat loss from the melt)
106 -cosl7.66°
AT with the values Zc = 3.84 kW, ZFLT = 1.56 kW and th = 41.8 kg/h from the earlierexample from Equation 5.50
Stock temperature at the outlet of the screw increment considered Tout:
T o u t = r M + 152.4 0C
Melting point of the polymer TM = 110 0C
Hence, Tout =110 + 152.4 = 262.4 0C
Average stock temperature T :
As already mentioned, this result can only be an estimate because the effect of the changeof temperature on the viscosity can be calculated only through an iterative procedure asshown in [9].
5.2.2.5 Melt Pressure
For a screw zone of constant depth the melt or stock pressure can generally be obtainedfrom the pressure flow by means of Equation 5.29. However, the following empiricalequation [10] has been found to give good results in practice:
(5.51)
(5.52)
The sign of Ap corresponds to that of the pressure flow Q p .
where
Example with symbols and units
a) Screw zone of constant channel depth (metering zone)
Empirical factor P 1 = 0.286Melt viscosity in screw channel 7]a = 1400 Pa • sShear rate in channel y = 84 s"1
Length of screw zone (or of an increment) A/ = 600 m mHelix angle <p =17.66°Channel depth at the outlet of the zone or increment Hout = 3 mmFlight clearance <5pL T =0.1 mmPressure flow Qp = 1.249 • 10 6 m3/sReciprocal of the power law exponent n nR - 0.5Ratio of channel depths at the outlet (Hout)and inlet (H1n) of the zone or increment HR HR = 1 (constant depth)Width of the channel W = 51.46 mmThickness of the melt film S{ = 0Number of flights V = 1
rjp from Equation 5.52:
Ap from Equation 5.51:
b) Screw zone of varying depth (transition zone)
H1n = 9 mm; Hout = 3 mm; A/ = 240 mm; T] = 1800 Pa • s; y = 42 s"1
rjp from Equation 5.52:
%= pT = 11665
Ap from Equation 5.51:
A more exact calculation of the melt pressure profile in an extruder should consider theeffect of the ratio of pressure flow to drag flow, the so called drossel quotient, as shown in[10].
5.2.3 Melting of Solids
Physical models describing the melting of solids in extruder channels were developed bymany workers, notably the work of TADMOR [6]. RAUWENDAAL summarizes the theoriesunderlying these models in his book [8], Detailed computer programs for calculatingmelting profiles based on these models have been given by RAO in his books [3, 9].
The purpose of the following section is to illustrate the calculation of the main parametersof these models through numerical examples. The important steps for obtaining a meltingprofile are treated in another section for a quasi Newtonian fluid.
5.2.3.1 Thickness of Melt Film
According to the Tadmor model [6] the maximum, thickness of the melt film (Figure 5.23)is given by
(5.53)
Example with symbols and units
Thermal conductivity of the melt Xm =0.174 W/(m K)Barrel temperature Th =150 0CMelting point of the polymer Tm = 110 0CViscosity in the melt film rjf Pa • sShear rate in the film fi s~l
Velocity of the barrel surface Vb cm/sVelocity components Vbx, Vbz cm/s (Figure 5.24)Velocity of the solid bed V 8 2 cm/sOutput of the extruder G_ = 16.67 g/sAverage film thickness S^ m mTemperature of the melt in the film Tf
0CAverage film temperature Ta
0CDepth of the feed zone H 1 = 9 mmWidth of the screw channel W = 51.46 mmMelt density p m = 0.7 g/cm3
Density of the solid polymer p s = 0.92 g/cm3
Specific heat of the solid polymer cps = 2.2 kj/(kg • K)Temperature of the solid polymer T5 = 20 0 CHeat of fusion of the polymer im =125.5 kj/kgMaximum film thickness < 5 m a x cm
Indices:
m: melts: solid
Figure 5.24 Velocity and temperature profiles in the melt and solid bed after TADMOR [6]a: solid melt interface, b: cylinder, c: solid bed
Following conditions are given:
The resin is LDPE with the same constants of viscosity as in Example 1 of Section 4.1.1.4.
The barrel diameter Db is 60 mm and the screw speed is 80 rpm.
Y
X-
Z
c
i f
b
Figure 5.23 Temperature profile in the melt film after TADMOR [6]a: solid bed, b: barrel surface, c: melt film, d: solid melt interface
y
Th
sy^sy
V
bXbCd
Q
Relative velocity Vj (Figure 5.24):
Temperature Ta:
Starting from an assumed film thickness of 0.1 mm and using the temperature resultingwhen heat generation is neglected, the viscosity in the film is estimated first. By changingthe film thickness and repeating this calculation, the final viscosity is obtained [3],
This iteration leads to
5max from Equation 5.53
Temperature in Melt Film
Taking the viscous heat generation into account, the temperature in melt film can beobtained from [6]
(5.54)
As seen from the equations above, the desired quantities have to be calculated on aniterative basis. This is done by the computer program given in [3].
5.2.3.2 Melting Rate
The melting rate is described by TADMOR [6] by the parameter <f>?, which is expressed as
(5.55)
The numerator represents the heat supplied to the polymer by conduction through thebarrel and dissipation, whereas the denominator shows the enthalpy required to meltthe solid polymer. The melting rate increases with increasing 0p .
By inserting the values given above into Equation 5.55 we obtain
5.2.3.3 Dimensionless Melting Parameter
The dimensionless melting parameter y/is defined as [6]
(5.56)
with
0n - 0.035 g/(cmL5 • s)H1 = 9 mmW = 51.46 mmG = 16.67 g/s
we get
The dimensionless parameter is the ratio between the amount of melted polymer perunit down channel distance to the extruder output per unit channel feed depth.
5.23.4 Melting Profile
The melting profile provides the amount of unmelted polymer as a function of screwlength (Figure 5.25) and is the basis for calculating the stock temperature and pressure.It thus shows whether the polymer at the end of the screw is fully melted. The plasticatingand mixing capacity of a screw can be improved by mixing devices. Knowledge of themelting profile enables to find the suitable positioning of mixing and shearing devices inthe screw [21].
The following equation applies to a screw zone of constant depth [6]
(5.57)
and for a tapered channel [6]
(5.58)
(5.59)
where
X/W
A/G
Figure 5.25 Solid bed or melting profiles X/W and Gs/G [21 ]G: total mass flow rate, G5: mass flow rate of solids
Cross-section of screw channelAxial distance along the screw
WX
Barrel
Screw
Melt Solid bed Melt film
XW
t
Figure 5.26 Three-zone screw [8]
The parameter yns obtained from Equation 5.56.
Symbols and units:
Xout, X1n mm Width of the solid bed at the outlet and inlet of a screw incrementrespectively
W mm Channel width\j/ Melting parameterAz mm Downchannel distance of the incrementH1n, Hout mm Channel depth at the inlet and outlet of an incrementH1, H2 mm Channel depth of a parallel zone (feed zone) and depth
at the end of a transition zone (Figure 5.26)A Relative decrease of channel depth, Equation 5.59Z mm Downchannel length of a screw zone
Example
a) Constant channel depth
For
H1 = 9 mm; XJW = 1; Az = 99 mm and y/= 0.004 from Section 4.2.3.3, Xout/Wcan becalculated from Equation 5.57:
This means that at a distance of Az = 99 mm, 4% of the solids were melted.
b) Varying channel depth
For the values
H1 = 9 mmH2 = 3 mmZ = 1584 mmXJW =0.96H1n = 9 m mH o u t = 8.625
Q b c
hMi
l/Acan be obtained from Equation 5.56:
The relative decrease of the channel depth A is calculated from Equation 5.59:
and Xout/W from Equation 5.58
Assuming a constant velocity of the solid bed, the mass flow ratio GJG results from
(5.60)
where
Gs = mass flow rate of the solid polymer g/sG = througput of the extruder g/sX = average OfX1n and Xout mmH = average of Hout, and H1n mm
For a zone of constant depth it follows that
(5.61)
a) Constant depth
b) Varying depth
The profiles of stock temperature and pressure can be calculated from the melting profileby using the width of the melt-filled part of the channel in the equations given inSection 5.2.2 [10].
5.2.4 Temperature Fluctuation of Melt
Temperature and pressure variations of the melt in an extruder serve as a measure for thequality of the extrudate and provide information as to the performance of the screw.
The temperature variation AT may be estimated from the following empirical relation,which was developed from the results of SQUIRES' experiments [12] conducted with 3-zonescrews:
This relation is valid for 0.1 K NQ < 0.5.
The parameter NQ is given by
(5.62)
(5.63)
where
AT= temperature variation (0C)Dh = barrel diameter (cm)G = extruder output (g/s)L = length of screw zone in diametersH - depth of the screw zone (cm)
Example
Following values are given:
Dh - 6 cmG = 15 g/s
L depth cm LIH
9 0.9 103 0.6 (mean value) 3.339 0.3 30
Hence
NQ from Equation 5.63:
AT from Equation 5.62:
The constants in the Equation 5.62 and Equation 5.63 depend on the type of polymerused. For screws other than 3-zone screws the geometry term in Equation 5.63 has to bedefined in such a way that NQ correlates well with the measured temperature fluctuations.
5.2.5 Scale-up of Screw Extruders
Based on the laws of similarity, PEARSON [13] developed a set of relationships to scale-upa single screw extruder. These relations are useful for the practicing engineer to estimatethe size of a larger extruder from experimental data gathered on a smaller machine. Thescale-up assumes equal length to diameter ratios between the two extruders. Theimportant relations can be summarized as follows:
(5.64)
(5.65)
(5.66)
(5.67)
where
HF = feed depthH = metering depthD = screw diameterN" = screw speed
Indices: 1 = screw of known geometry and 2 = screw to be determined.
The exponent s is given by
where nR is the reciprocal of the power law exponent n. The shear rate required todetermine n is obtained from
Example
Following conditions are given:
The resin is LDPE with the same constants of viscosity as in Example 1 of Section 5.1.1.4.The stock temperature is 200 0C. The data pertaining to screw 1 are:
D1 = 90 mm; HF = 12 mm; H1 = 4 mm
feed length = 9 D1
transition length =2 D1
metering length =9 D1
output Ih1 = 130kg/hscrew speed N1 = 80 rpm
The diameter of screw 2 is D2 = 120 mm. The geometry of screw 2 is to be determined.
Solution
The geometry is computed from the equations given above [3]. It follows that
D2 = 1 2 0 mmHp2 = 14.41mmH2 = 4.8 mmm2 = 192.5 kg/hN1 = 55.5 rpm
Other methods of scaling up have been treated by SCHENKEL [29], FENNER [30], FISCHER
[31],andPoTENTE [32].
Examples for calculating the dimensions of extrusion screws and dies are illustrated inthe following figures:
Spec
ific
outp
ut k
g/h/
rpm
Extru
der o
utpu
t (kg
/h)
Screw diameter D (mm)
Figure 5.27 Specific output vs. screw diameter for LDPE and LLDPE (UD = 20)
LLDPEpower law
exponent n = 2
LDPEpower lawexponent n = 2.5
Screw diameter D (mm)
Figure 5.28 Extruder output vs. screw diameter for LDPE (UD = 20)
Scre
w s
peed
(rp
m)
Moto
r pow
er (k
W)
Screw diameter D (mm)Figure 5.29 Screw speed vs. screw diameter for LDPE [UD = 20)
Screw diameter D (mm)Figure 5.30 Motor power vs. screw diameter for LDPE [UD = 20)
Pres
sure
dro
p (b
ar)
Pres
sure
dro
p (b
ar)
Chan
nel d
epth
H (m
m)
Die gap H (mm)Figure 533 Pressure drop vs. die gap for PET
PET
Flow rate= 36 kg/h
T = 3000C
T = 2800C
Die gap H (mm)Figure 5.32 Pressure drop vs. die gap for a flat die
Flow rate= 36 kg/h
LLDPET = 250°C
LDPET = 200°C
Screw diameter (mm)Figure 5.31 Channel depth vs. screw diameter for LDPE [UD = 20)
LDPEpower lawexponentn = 2.5
metering depth
feed depth
5.2.6 Mechanical Design of Extrusion Screws
5.2.6.1 Torsion
The maximum shear stress Tmax, which occurs at the circumference of the screw root as aresult of the torque MT, is given by [8]
(5.68)
where I? = root radius of the screw.
The maximum feed depth Hmax can be computed from [8]
(5.69)
where
D = diameterTzul = allowable shear stress of the screw metal
Example [8]
The maximum feed depth is to be calculated for the following conditions:
D = 150 mm; M x = 17810 Nm; Tzul = 100 MPa;
Hmax is found from Equation 5.69:
5.2.6.2 Deflection
Lateral Deflection
The lateral deflection of the screw (Figure 5.34) caused by its own weight can be obtainedfrom [8]
(5.70)
Figure 5.34 Lateral deflection of the screw as cantilever [8]
Numerical example with symbols and units [8]
g =9.81 m2/s acceleration due to gravityp = 7850 kg/m3 density of the screw metalL = 3 m length of the screwE - 210 • 109 Pa elastic modulus of the screw metalD = 0.15 m screw diameter
Inserting these values into Equation 5.70 we get
This value exceeds the usual flight clearance, so that the melt between the screw and thebarrel takes on the role of supporting the screw to prevent contact between the screw andthe barrel [8].
Buckling Cuased by Die Pressure
The critical die pressure, which can cause buckling, can be calculated from [8]
(5.71)
Numerical example [8]
E = 210 • 109 Pa elastic modulus of the screw metalLID = 35 length to diameter ratio of screw
pK from Equation 5.71:
As can be seen from Equation 5.71, the critical die pressure pK decreases with increasingratio LID. This means, that for the usual range of die pressures (200-600 bar) bucklingthrough die pressure is a possibility, if the ratio LID exceeds 20 [8].
/U)
L
Screw Vibration
When the screw speed corresponds to the natural frequency of lateral vibration of theshaft, the resulting resonance leads to large amplitudes, which can cause screw deflection.The critical screw speed according to [8] is given by
(5.72)
Substituting the values for steel, E = 210 • 109 Pa and p = 7850 kg/m3 we get
(5.73)
Numerical example
For D = 150 mm and — = 30, NR is found from Equation 5.73
This result shows that at the normal range of screw speeds vibrations caused by resonanceare unlikely.
Uneven Distribution of Pressure
Non-uniform pressure distribution around the circumference of the screw can lead tovertical and horizontal forces of such magnitude, that the screw deflects into the barrel.Even a pressure difference of 10 bar could create a horizontal force Fj1 in an extruder(diameter D = 150 mm within a section of length L = 150 mm)
According to RAUWENDAAL [8], the non uniform pressure distribution is the most probablecause of screw deflection.
5 3 Injection Mo ld ing
Other than extrusion, injection molding runs discontinuously and therefore the stagesinvolved in this process are time-dependent [14]. The quantitative description of theimportant mold filling stage has been made possible by well known computer programssuch as MOLDFLOW [15] and CADMOULD [16]. The purpose of this section is topresent the basic formulas necessary for designing injection molding dies and screws ona rheological and thermal basis and illustrate the use of these formulas with examples.
Next Page
Screw Vibration
When the screw speed corresponds to the natural frequency of lateral vibration of theshaft, the resulting resonance leads to large amplitudes, which can cause screw deflection.The critical screw speed according to [8] is given by
(5.72)
Substituting the values for steel, E = 210 • 109 Pa and p = 7850 kg/m3 we get
(5.73)
Numerical example
For D = 150 mm and — = 30, NR is found from Equation 5.73
This result shows that at the normal range of screw speeds vibrations caused by resonanceare unlikely.
Uneven Distribution of Pressure
Non-uniform pressure distribution around the circumference of the screw can lead tovertical and horizontal forces of such magnitude, that the screw deflects into the barrel.Even a pressure difference of 10 bar could create a horizontal force Fj1 in an extruder(diameter D = 150 mm within a section of length L = 150 mm)
According to RAUWENDAAL [8], the non uniform pressure distribution is the most probablecause of screw deflection.
5 3 Injection Mo ld ing
Other than extrusion, injection molding runs discontinuously and therefore the stagesinvolved in this process are time-dependent [14]. The quantitative description of theimportant mold filling stage has been made possible by well known computer programssuch as MOLDFLOW [15] and CADMOULD [16]. The purpose of this section is topresent the basic formulas necessary for designing injection molding dies and screws ona rheological and thermal basis and illustrate the use of these formulas with examples.
Previous Page
5.3.1 Pressure Drop in Runner
As the following example shows, the pressure drop along the runner of an injection moldcan be calculated from the same relationships used for dimensioning extrusion dies.
Example
For the following conditions, the isothermal pressure drop Ap0 and the adiabatic pressuredrop Ap are to be determined:
For polystyrene with the following viscosity constants according to Equation 1.36,Section 1.3.7.3:
A0 = 4.4475A1 = -0.4983A2 = -0.1743A3 = 0.03594A4 = -0.002196C1 = 4.285C2 =133.2T0 = 190 0C
flow rate rh = 330.4 kg/hmelt density p m = 1.12 g/cm3
specific heat cpm= 1.6 kj/(kg • K)melt temperature T =230 0Clength of the runner L =101.6 mmradius of the runner R =5.08 mm
Solution
a) Isothermal flow
Yz from Equation 1.19:
(Q = volume flow rate cm /s)
aT from Equation 1.35:
n from Equation 1.37:
7]a from Equation 1.36:
In the adiabatic case, the pressure drop is smaller because the dissipated heat is retainedin the melt.
T from Equation 1.22:
T= 105013.6 Pa
K from Equation 1.26:
Die constant Gcirde from Equation 5.3:
Ap0 with Q = 8.194 • 10 5 m3/s from Equation 5.2:
b) Adiabatic flow
The relationship for the ratio —— is [17]Ap0
(5.74)
(5.75)
where
Temperature rise from Equation 5.18:
For polystyrene
Finally, Ap from Equation 5.74:
Examples of calculating pressure drop in runners of different geometry are shown in thefollowing figures:
Pres
sure
dro
p (ba
r)Pr
essu
re d
rop
(bar
)Pr
essu
re D
rop
(bar
)
LDPET = 2000CL = 100 mm
Flow rate (kg/h)
Figure 5.35 Pressure drop vs. flow rate for a circular cross-section for LDPE
Flow rate (kg/h)
Figure 5.36 Effect of melt viscosity on pressure drop
R = 3 mmT = 2700CL = 100 mm
Flow Rate (kg/h)
Figure 5.37 Effect of channel shape on pressure drop
LDPET = 27O0CL = 100 mmR = 3.39 mm
R
R
R
Flow rate (kg/h)
Figure 5.38 Pressure drop for a noncircular channel with /?rh = 2.77 mm and n = 2.052
53.2 Mold Filling
As already mentioned, the mold filling process is treated extensively in commercialsimulation programs [15,16] and recently by BANGERT [18]. In the following sections themore transparent method of STEVENSON [19] is given with an example.
53.2.1 Injection Pressure and Clamp Force
To determine the size of an injection molding machine for the production of a givenpart, knowledge of the clamp force exerted by the mold is important, because this forceshould not exceed the clamp force of the machine.
Injection Pressure
The isothermal pressure drop for a disc-shaped cavity is given as [19]
(5.76)
(5.77)
(5.78)
The fill time T is defined as [19]
The Brinkman number is given by [19]
Pres
sure
dro
p (b
ar)
LDPET = 2700CL = 100 mm
R=3mm
62
Example with symbols and units
The material is ABS with nR = 0.2565, which is the reciprocal of the power law exponentn. The constant K1, which corresponds to the viscosity T]p in Equation 5.52 is K1 = 3.05 • 104.
Constant injection rate Q =160 cm3/sPart volume V = 160 cm3
Half thickness of the disc b =2.1 mmRadius of the disc r2 =120 mmNumber of gates N=IInlet melt temperature TM = 518 KMold temperature T w = 323 KThermal conductivity of the melt /L = 0.174 W/(m • K)Thermal difrusivity of the polymer a = 7.72 • 10 cm /sMelt flow angle [19] 0 = 360°
The isothermal pressure drop in the mold Ap1 is to be determined.
Solution
Applying Equation 5.76 for Ap1
Dimensionless fill time T from Equation 5.77:
Brinkman number from Equation 5.78:
From the experimental results of STEVENSON [19], the following empirical relation wasdeveloped to calculate the actual pressure drop in the mold
(5.79)
The actual pressure drop Ap is therefore from Equation 5.79:
Clamp Force
The calculation of clamp force is similar to that of the injection pressure. The isothermalclamp force is determined from [19]
(5.80)
where F1(T2) = isothermal clamp force (N).
F1(T2) for the example above is with Equation 5.80
The actual clamp force can be obtained from the following empirical relation, which wasdeveloped from the results published in [19].
(5.81)
Hence the actual clamp force F from Equation 5.81
The above relationships are valid for disc-shaped cavities. Other geometries of the moldcavity can be taken into account on this basis in the manner described by STEVENSON
[19].
5.3.3 Flowability of Injection Molding Resins
The flowability of injection molding materials can be determined on the basis of meltflow in a spiral channel. In practice, a spiral-shaped mold of rectangular crosssectionwith the height and width in the order of a few millimeters is often used to classify theresins according to their flowability. The length L of the solidified plastic in the spiral istaken as a measure of the viscosity of the polymer concerned.
Figure 5.39 shows the experimentally determined flow length L as a function of the heightH of the spiral for polypropylene. A quantitative relation between L and the parametersinfluencing L such as type of resin, melt temperature, mold temperature, and injectionpressure can be developed by using the dimensionless numbers as defined by THORNE
[23] in the following manner:
The Reynolds number Re is given by [23]
(5.82)
(5.83)
where
As shown in [20] and in Figure 5.40, the Graetz number correlates well with the productRe-Pr- Br
(5.87)
An explicit relationship for the spiral length L can therefore be computed from thiscorrelation.
Flow
length
L
PP
mm
mm
(5.84)
(5.85)
(5.86)
Spiral height HFigure 5.39 Flow length L as a function of the spiral height H
Prandtl number Pr [23]
and Brinkman number Br [23]
In addition, the Graetz number is defined by
Figure 5.40 Dimensionless groups for determining the flowability of a resin [20]
Symbols and units:
Br Brinkman numbercp Specific heat kj/(kg • K)Y Apparent shear rate s"1
G Mass flow rate kg/hGz Graetz numberJFf Height of the spiral m mH Half height of the spiral m mk Constant from Equation 5.83L Length of the spiral m mnR Reciprocal of the power law exponentPr Prandtl numberQ Volume flow rate m3/sRe Reynolds numberTM Melt temperature 0CT w Mold temperature 0CV6 Velocity of the melt front m/sW Width of the spiral m mA Thermal conductivity W/(m • K)p Melt density g/cm?]a Melt viscosity Pa*s
Example
This example illustrates the calculation of the dimensionless numbers Gz, Re, Pr and Brfor:
W=IO mm; H = I mm; L = 420 mm; p = 1.06 g/cm3; cp = 2 kj/(kg • K);X = 1.5 W/(m • K); TM = 270 0C; Tw = 70 0C; G = 211.5 kg/h
Resin-dependent constants according to Equation 1.36:
A0 = 4.7649; A1 = 0.4743; A2 = 0.2338; A3 = 0.081; A4 = 0.01063;C1 = 4.45; C2 = 146.3; T0 = 190 0C
Grae
tz nu
mber
Gz
RePrBr
Solution
The conversion factors for the units used in the calculation of the dimensionless numbersbelow are
F1 = 0.001; F2 = 1000; F3=3600
The Graetz number Gz is calculated from
with G in kg/h and L in mm. Using the values given above, Gz =186.51. The Reynoldsnumber is obtained from
with Ve in m/s, H* in m and p in g/cm3.
Using the values given above, Re = 0.03791.
With H in m and Ve in m/s we get from
and the Brinkman number Br from
Finally, the product Re • Pr • Br = 7768.06.
5.3.4 Cooling of Melt in Mold
As mentioned in Section 3.2.1, the numerical solution of the Fourier equation, Equation3.31, is presented here for crystalline and amorphous polymers.
5.3.4.1 Crystalline Polymers
The enthalpy temperature diagram of a crystalline polymer shows that there is a sharpenthalpy rise in the temperature region where the polymer begins to melt. This is causedby the latent heat of fusion absorbed by the polymer when it is heated and has to betaken into account when calculating cooling curves of crystalline polymers.
By defining an equivalent temperature for the latent heat (Figure 5.41), GLOOR [22]calculated the temperature of a slab using the Fourier equation for the non-steady-state
Figure 5.41 Representation of temperature correction for latent heat [22]
heat conduction. The numerical solution of Equation 3.31 using the correction introducedby GLOOR [22] was given in [25] on the basis of the method of differences after SCHMIDT
[24]. A computer program for this solution is presented in [3]. The time interval used inthis method is
(5.88)
where
At = time intervalAx = thickness of a layerM = number of layers, into which the slab is devided, beginning from the mid plane of
the slab (Figure 5.42)
The mold temperature and the thermodynamic properties of the polymer are assumedto be constant during the cooling process. The temperature at which the latent heat isevolved, and the temperature correction W1 (Figure 5.41) are obtained from the enthalpydiagram as suggested by GLOOR [22]. An arbitrary difference of about 6 0C is assignedbetween the temperature of latent heat release at the mid plane and the temperature atthe outer surface of the slab.
Entha
lpy
Temperature T
Figure 5.42 Nomenclature for numerical solution of non-steady state conduction in a slab [25]
s
Temp
eratu
re T
Temp
eratu
re J
Figure 5.43 Plot of mid plane temperature vs. time for a crystalline polymerTime /
Figure 5.43 shows a sample plot of temperature as a function of time for a crystallinepolymer.
0C
s
0C
s
Figure 5.44 Plot of mid plane temperature vs. time for an amorphous polymerTime/
5.3.4.2 Amorphous Polymers
Amorphous polymers do not exhibit the sharp enthalpy change as crystalline plasticswhen passing from liquid to solid. Consequently, when applying the numerical methodof SCHMIDT [24], the correction for the latent heat can be left out in the calculation.A sample plot calculated with the computer program given in [3] is shown in Figure 5.44for amorphous polymers.
It is to be mentioned here that the analytical solutions for non-steady heat conductiongiven in Section 3.2.1 serve as good approximations for crystalline as well as foramorphous polymers.
5.3.5 Design of Cooling Channels
5.3.5.1 Thermal Design
In practice, the temperature of the mold wall is not constant, because it is influenced bythe heat transfer between the melt and the cooling water. Therefore, the geometry of thecooling channel lay out, the thermal conductivity of the mold material, and the velocityof the cooling water affect the cooling time significantly.
The heat transferred from the melt to the cooling medium can be expressed as (Figure5.45)
(5.89)
The heat received by the cooling water in the time tK amounts to
(5.90)
The cooling time tK in this equation can be obtained from Equation 3.41. The influenceof the cooling channel lay out on heat conduction can be taken into account by the shapefactor Se according to [23, 26].
Figure 5.45 Geometry for the thermal design of cooling channels
The mold temperature Tw in Equation 3.41 is calculated iteratively from the heat balance
Qab=Qw
Example with symbols and units
Part thickness s =2 mmDistance x = 30 mmDistance y = 1 0 m mDiameter of cooling channel d — 10 mmMelt temperature TM = 250 0CDemolding temperature TE = 90 0CLatent heat of fusion of the polymer im =130 kj/kgSpecific heat of the polymer cps = 2.5 kj/(kg • K)Melt density p m = 0.79 g/cm3
Thermal diffusivity of the melt a = 8.3 • 10"4 Cm2IsKinematic viscosity of cooling water V = 1.2 • 10"6 m2/sVelocity of cooling water u = 1 m/sTemperature of cooling water ^water - 15 0CThermal conductivity of mold steel Ast = 45 W/(m • K)
With the data above the heat removed from the melt Qab according to Equation 5.89 is
(5.91)
(5.92)
With the values for the properties of water
the heat transfer coefficient a can be obtained from Equation 3.52
Reynolds number of water:
Using Equation 5.92 for the heat transfer coefficient a
From Equation 5.90 we get for the heat received by the cooling water Qw
Cooling time tK from Equation 3.41:
From the heat balance
we obtain by iteration
Tw = 37.83 0C
Finally, the cooling time tK with Tw = 37.83 is from Equation 3.41
tK = 8.03 s
The influence of the cooling channel lay out on cooling time can be simulated on thebasis of the equations given by changing the distances x and y (Figure 5.45) as shownin Figure 5.46 and Figure 5.47. The effects of the temperature of cooling water and ofits velocity are presented in Figure 5.48 and Figure 5.49, respectively. From these resultsit follows that the cooling time is significantly determined by the cooling channel layout.
Shape factor Se from Equation 5.91:
Cooli
ng t
ime
Cooli
ng ti
meCo
oling
time
Cooli
ng t
ime
Distance between mold surface and cooling channel YFigure 5.46 Effect of cooling channel distance y on cooling time
mm
s 7 =2O0C
W=io°c
s 7WaIeT=2000
W = ^ O 0 C
mm
Distance from channel to channel /
F i g u r e 5 . 4 7 Ef fect o f c o o l i n g c h a n n e l d i s t a n c e x o n c o o l i n g t i m e
s
5 = 1.5 mm/ = 2 5 mmK= 15 mm
0C
Cooling water temperature
F i g u r e 5 . 4 8 I n f l u e n c e o f t h e t e m p e r a t u r e o f c o o l i n g w a t e r o n c o o l i n g t i m e
s
Velocity of cooling water
F i g u r e 5 . 4 9 I n f l u e n c e o f t h e v e l o c i t y o f c o o l i n g w a t e r o n c o o l i n g t i m e
m/s
S= 1.5mm
/ = 2 5 mm
K = 1 5 m m
W 2 0 ° C
5.3.5.2 Mechanical Design
The cooling channels should be as close to the surface of the mold as possible so that heatcan flow out of the melt in the shortest time possible.
Figure 5.50 Geometry for the mechanical design of cooling channels
However, the strength of the mold material sets a limit to the distance between the coolingchannel and the mold surface. Taking the strength of the mold material into account, theallowable distance d (Figure 5.50) was calculated by [27] on the basis of the followingequations:
(5.93)
(5.94)
(5.95)
where
p = mold pressure N/mm2
/, d - distances mm, see Figure 5.50E = tensile modulus N/mm2
G = shear modulus N/mm2
<7h - allowable tensile stress N / m m 2
Tmax = allowable shear stress N / m m 2
/max ~ m a x - deflection of the m o l d material above the cooling channel |LLm
The minimizat ion of the distance d such that the condi t ions
are satisfied, can be accomplished by the compute r p rog ram given in [3]. The results of asample calculation are shown Table 5.2.
Mold surface
d
I
The equations given provide approximate values for circular channels as well. The distancefrom wall to wall of the channel should be approximately the channel length / or channeldiameter, taking the strength of the mold material into account.
53.6 Melting in Injection Molding Screws
The plastication of solids in the reciprocating screw of an injection molding machine isa batch process and consists of two phases. During the stationary phase of the screwmelting takes place mainly by heat conduction from the barrel. The melting during screwrotation time of the molding cycle is similar to that in an extrusion screw but instationary.With long periods of screw rotation, it approaches the steady state condition of extrusionmelting.
5.3.6.1 Melting by Heat Conduction
According to DONOVAN [28], the equation describing conduction melting can be written as
Table 5.2 Results of Optimization of Cooling Channel Distance in Figure 5.50
Input
Mold pressureMaximum deflectionModulus of elasticityModulus of shearAllowable tensile stressAllowable shear stressChannel dimension
P - 4.9 N/mm2
/max = 2.5 Umj T = 70588 N/mm2
G = 27147 N/mm2
ah =421.56 N/mm2
Dmax ,
Tmax =294.1 N/mm/ = 10 m m
Output
Channel distanceDeflectionTensile stressShear stress
d =2.492 mm/ = 2.487 umG =39.44 N/mm2
T = 14.75 N/mm2
(5.96)
where
T = temperature 0CA = thermal conductivity W/(m • K)K = Parameter defined by [28] m/s0*5
a = thermal diffusivity m2/sI = latent heat of fusion kj/kgp = density g/cm3
Indices:
r: middle of solid beds: solidm: meltb: barrel
The parameter K can be determined iteratively by means of the computer program givenin [9].
5.3.6.2 Melting during Screw Rotation
Analogous to the melting model of Tadmor (Section 4.2.3), DONOVAN [28] defines anarea ratio A
to quantitatively describe the melting or solid bed profile of a reciprocating screw. A isthe ratio of the cross-sectional area of solid bed As to the cross sectional area of screwchannel Ax.
The equations according to DONOVAN [28] for calculating the solid bed profiles are asfollows:
(5.97)
(5.98)
(5.99)
where
tT = total cycle time stR = screw rotation time s4 = thickness of melt film mH = depth of the screw channel mb = dimensionless parameterN = screw speed rpm
Indices:
i: beginning of screw rotationf: end of screw rotatione: extrusion
Axial distance along the screw
Figure 5.51 Solid bed profile of an injection molding screw
The thickness of the melt film <% and the solid bed profile for steady state extrusion Ae
can be obtained from the relationships in the Tadmor model given in Section 4.2.3.
The area ratio at the start of screw rotation A1 and the value at the end of screw rotationAf can then be obtained by using the computer program given in [9]. Figure 5.51 showsthe solid bed profiles of a computer simulation [9] for a particular resin at given operatingconditions.
Calculation procedure
Step 1: Calculate K using Equation 5.96.
Step 2: Calculate Say according to
The average temperature in the melt film is obtained from
Substitute 8{ with <5av.
Step 3: Calculate the solid bed ratio A* for steady-state extrusion with the simplifiedmodel for a linear temperature profile.
Step 4: Find the solid bed ratio Af at the end of the screw rotation using Equation 5.97and Equation 5.98.
Step 5: Calculate A1*, the solid bed ratio at the start of screw rotation from Equation 5.99.
Per
cent
unme
lted
A6 ^ = IOOmJn"1
4 /T=30sA1 fR=4.8s
%
The following sample calculation shows the symbols and units of the variables occurringin the equations above.
Example
The thermal properties for LDPE and the barrel temperature are as given in the previouscalculation for the parameter K. In addition,
Total cycle time tT = 45 sScrew rotation time tR = 22 sEmpirical parameter for all polymers /J = 0.005Screw speed N = 56 rpmChannel depth H = 9.8 mmChannel width W = 52.61 mmCross-channel velocity of the melt vbx = 5.65 cm/sRelative velocity of the melt v; = 15.37 cm/sSolids temperature Ts =20 0C
By using these values and by iteration, the following target values are obtained:
Melt viscosity in the film 7]f = 211 Pa • sAverage temperature of the melt in the film Tf = 172.8 0CAverage thickness of the melt film <5av = 7.678 10" cm
Using K = 5.6 • 10"4, the solid bed ratios are found to be: the solid bed ratio at the end ofscrew rotation, A*{ = 0.583; the solid bed ratio at the start of screw rotation, A1* = 0.429.The solid bed ratio for steady-state extrusion, Ae, is calculated from the simplified meltingmodel for extrusion. Its numerical value for the conditions above is Ae = 0.75.
In the following figures the steady-state extrusion profile begins at the position of thestroke. The temperature of the melt refers to the temperature at the end of the screwfor the case of steady-state extrusion. The solid bed ratio A is the ratio between thecross-sectional area of the solid bed As and the total cross-sectional area of the channelAx. In Figure 5.52 the effect of the resin type on the solid bed profiles is presented. Itappears that the conductivity parameter K and the melt viscosity affect these profilessignificantly, even if the screw rotation and cycle times remain the same. It can be seenfrom Figure 5.53 that the barrel temperature has little effect on the plastication processin the screw.
As Figure 5.54 depicts, slow screw speed and a high percentage of screw rotation timecompared to total cycle time favor melting strongly, which has also been found by Donovan[28]. The marked influence of screw geometry on melting becomes clear from Figure 5.55.As can be expected, melting is much faster in a shallower channel.
Figure 5.52 Effect of polymer on the melting profiles
Axial length (screw diameters)
Screw profileA* [%]
LDPE
Extrusion melttemperature Tm
Tm
Axial length (screw diameters)
Screw profile
A* [%] Tm
PP
Axial length (screw diameters)
Screw profile
A*[%] Tm
PA66
Screw profile
Screw profile
Screw profile
Screw profileTm
Tm
Tm
7m
Extrusion melttemperature Tm
Extrusion melttemperature Tm
LDPE
LDPE
PP
PP
A* [%]
A* [%]
A* [%)
A* [%]
Figure 5.53 Effect of barrel temperature on the melting profile for PP
Axial length (screw diameters)
Axial length (screw diameters)
Figure 5.54 Effect of screw rotation time and screw speed on melting of LDPE
Axial length (screw diameters)
Axial length (screw diameters)
Figure 5.55 Effect of screw geometry on the melting for LDPE
53.7 Predicting Flow Length of Spiral Melt Flows
Injection molding is widely used to make articles out of plastics for various applications.One of the criteria for the selection of the resin to make a given part is whether the resinis an easy flowing type or whether it exhibits a significantly viscous behavior. To determinethe flowability of the polymer melt, the spiral test, which consists of injecting the meltinto a spiral shaped mold shown in Figure 5.56, is used. The length of the spiral serves asa measure of the ease of flow of the melt in the mold and enables mold and part designappropriate for a specific material flow behavior.
Screw profile
Screw profilerm
7"mA* [%]
A* [%]
LDPE
Extrusion melttemperature Tm
LDPE
Axial length (screw diameters)
Axial length (screw diameters)
Cross sectionFigure 5.56 Schematic representation of spiral form
w
H
Spiral height H
Figure 5.57 Schematic flow curves
The experimental flow curves obtained at constant injection pressure under given melttemperature, mold temperature, and axial screw speed are given schematically inFigure 5.57 for a resin type at various spiral heights with melt flow index of the polymerbrand as parameter. By comparing the flow lengths with one another at any spiral height,also called wall thickness, the flowability of the resin in question with reference to anotherresin can be inferred.
The transient heat transfer and flow processes accompanying melt flow in an injectionmold can be analyzed by state-of-the-art commercial software packages. However, forsimple mold geometries, such as the one used in the spiral test, it is possible to predictthe melt flow behavior on the basis of dimensionless numbers and obtain formulas usefulin practice. These relationships can easily be calculated with a handheld calculator offeringquick estimates of the target values. Owing to the nature of non-Newtonian flow, thedimensionless numbers used to describe flow and heat transfer processes of Newtonianfluids have to be modified for polymer melts. As already presented in Section 5.3.3, themovement of a melt front in a rectangular cavity can be correlated by Graetz number,Reynolds number, Prandtl number, and Brinkman number. Because the flow length in aspiral test depends significantly on the injection pressure (Figure 5.58), the Euler number[41] is included in the present work in order to take the effect of injection pressure onthe flow length.
Flow
leng
th L
Increasing MFI
Flow
leng
th (m
m)
Flow
leng
th (m
m)
Flow
leng
th (m
m)
Flow
leng
th (m
m)
Flow
leng
th (m
m)
LDPE
Injection pressure (bar)
Figure 5.58 Effect of Injection pressure on flow length
In addition to the dimensionless numbers Gz, Re, Pr, and Br, we consider [41] the Eulernumber
(5.100)
where P1 is the injection pressure.
Experimental flow curves for four different resins measured at constant injection pressureunder different processing conditions and spiral wall thicknesses are given in Figure 5.59.
LDPE HDPE
PSPP
Injection pressure (bar) Injection pressure (bar)
Injection pressure (bar) Injection pressure (bar)
Figure 5.59 Experimental flow curves for LDPE, HDPE, PP, and PS
Figure 5.60 Graetz number as a function of the product of Re, Pr, Br, and Eu
The flow length as a function of injection pressure is shown in Figure 5.58 for LDPE asan example. The Graetz numbers calculated from the experimentally determined spirallengths at different operating conditions and resins are plotted as functions of the productRe • Pr • Br • Eu as shown in Figure 5.60. As can be seen from this figure, the correlationof the Graetz number with this product is good and thus for any particular material thespiral length can be predicted from the relationship
(5.101)
Figure 5.61 shows the good agreement between measured and calculated spiral lengthsfor the experimentally investigated resins.
Sample Calculation
The example given below shows how the flow length of a given resin can be calculated fromEquation 5.101: W= 10mm,H=2 mm,p= 1.06g/cm3,cp = 2kj/kg• K,X = 1.5 W/K• m,TM = 270 0C, Tw = 70 0C and G = 211.5 kg/h.
The melt viscosity rja is calculated from
Gra
etz
num
ber G
z
Gra
etz
num
ber
Gz
Gra
etz
num
ber G
z
Gra
etz
num
ber G
z
LDPE HDPE
PSPP
Re Pr Br Eu Re Pr Br Eu
Re Pr Br EuRe Pr Br Eu
Figure 5.61 Comparison between measured and calculated flow length ( calculated;D measured)
The shear rate y is obtained from
where Wmean = W + H • tana
A0, A1, A2, A3, A4 are material constants, and aT the shift factor. For amorphous polymersthe shift factor is obtained from
with constants C1, C2 and melt and reference temperatures T and T0, respectively, in K. Forsemi-crystalline and crystalline polymers ar is calculated from
with the constants bv b2 and melt temperature Tin K.
Using the values of A0 = 4.7649, A1 = -0.4743, A2 = -0.2338, A3 = 0.081, A4 = -0.01063,C1 = 4.45, C2 = 146.3 and T0 = 190 0C, the following output is obtained: Re = 0.05964,Pr = 76625.34, Br = 1.7419, and Eu = 10825.84. The Graetz number Gz for the productRe • Pr • Br • Eu follows from Figure 5.60: Gz = 217.63. Hence L = 420 mm.
Flow
leng
th L
(mm
)
Flow
leng
th L
(mm
)
Flow
leng
th L
(mm
)
Flow
leng
th L
(mm
)
LDPE HDPE
PSPP
Spiral height H (mm) Spiral height H (mm)
Spiral height H (mm) Spiral height H (mm)
References
[I] RAO, N.: EDV Auslegung von Extrudierwerkzeugen, Kunststoffe 69 (1979) 3, p. 226
[2] PROCTER, B.: SPE J. 28 (1972) p. 34
[3] RAO, N.: Designing Machines and Dies for Polymer Processing with Computer Programs,Hanser Publishers, Munich (1981)
[4] RAMSTEINER, R: Kunststoffe 61 (1971) 12, p. 943
[5] SCHENKEL, G.: Private Communication
[6] TADMOR, Z., KLEIN, L: Engineering Principles of Plasticating Extrusion, Van Nostrand Reinhold,New York (1970)
[7] BERNHARDT, E. C : Processing of Thermoplastic Materials, Reinhold, New York (1963)
[8] RAUWENDAAL, C : Polymer Extrusion, Hanser Publishers, Munich (2001)
[9] RAO, N.: Computer Aided Design of Plasticating Screws, Programs in Fortran and Basic,Hanser Publishers, Munich (1986)
[10] KLEIN, L, MARSHALL, D. I.: Computer Programs for Plastics Engineers, Reinhold, New York(1968)
[II] WOOD, S. D.: SPE 35, Antec (1977)
[12] SQUIRES, R H.: SPE J. 16 (1960), p. 267
[13] PEARSON, J. R. A.: Reports of University of Cambridge, Polymer Processing Research Centre(1969)
[14] JOHANNABER, E: Injection Molding Machines, Hanser Publishers, Munich (1994)
[16] CADMOULD: Project Rechnergestiitzte Formteil- and Werkzeugauslegung, IKV, Aachen
[17] MCKELVEY, J. M.: Polymer Processing, John Wiley, New York (1962)
[18] BANGERT, H.: Systematische Konstruktion von Spritzgiefiwerkzeugen unter Rechnereinsatz,Dissertation, RWTH Aachen (1981)
[19] STEVENSON, J. E: Polym. Eng. ScI 18 (1978) p. 573
[20] RAO, N.: Kunststoffe 73 (1983) 11, p. 696
[21] RAO, N., HAGEN, K., KRAMER, A.: Kunststoffe 69 (1979) 10, p. 173
[22] GLOOR, W. E.: Heat Transfer Calculations, Technical Papers, Volume IX-I, p. 1
[23] THRONE, I. L.: Plastics Process Engineering, Marcel Dekker, New York (1979)
[24] SCHMIDT, E.: Einfuhrung in die Technische Thermodynamik, Springer, Berlin (1962) p. 353
[25] MENGES, G., JORGENS, W: Plastverarbeiter 19 (1968) p. 201
[26] VDI Warmeatlas, VDI Verlag, Dusseldorf (1984)
[27] LINDNER, E.: Berechenbarkeitvon Spritzgiefiwerkzeugen, VDI Verlag, Dusseldorf (1974) p. 109
[28] DONOVAN, R. C : Polym. Eng. ScL 11 (1971) p. 361
[29] SCHENKEL, G.: Kunststoff-Extrudiertechnik. Hanser Publishers, Munich (1963)
[30] FENNER, R. T.: Extruder Screw Design. ILiFFE Books, London (1970)
[31] FISCHER, P.: Dissertation, RWTH Aachen (1976)
[32] POTENTE, H.: Proceedings, 9. Kunststofftechnisches Kolloquium, IKV, Aachen (1978)
[33] RAO, N. S.: Practical Computational Rheology Primer, Proc, TAPPI PLC (2000)
[34] SAMMLER, R. L., KOOPMANS, R. J., MAGNUS, M. A. and BOSNYAK, C. P.: Proc. ANTEC 1998, p. 957
(1998)
[35] ROSENBAUM, E. E. et al.: Proc, ANTEC 1998, p. 952 (1998)
[36] BASF Brochure: Blow molding (1992)
[37] Rao, N. S. and O'Brien, K.: Design Data for Plastics Engineers, Hanser Publishers, Munich(1998)
[38] BASF Brochure: Kunststoff Physik im Gesprach (1977)
[39] AGASSANT, J. F., AVENAS, P., SERGENT, J.Ph. and CARREAU, P. I.: Polymer Processing, Hanser
Publishers, Munich (1991)
[40] KAMAL, M. R., KERNIG, S.: Polym. Eng. ScL 12 (1972)
[41] PERRY,R. H., GREEN, D.: Perry's Chemical Engineer's Handbook, Sixth Edition, p. 2-116 (1984)
[42] CARLEY, J. E, SMITH W. C : Polym. Eng. ScL 18 (1978)
[43] Brochure of BASF AG, 1992
B i o g r a p h y
Natti S. Rao obtained his B.Tech(Hons) in Mechanical Engineering and M.Tech. inChemical Engineering from the Indian Institute of Technology, Kharagpur, India. Afterreceiving his Ph. D. in Chemical Engineering from the University of Karlsruhe, Germany,he worked for the BASF AG for a number of years. Later, he served as a technical advisorto the leading machine and resin manufacturers in various countries.
Natti has published over 60 papers and authored four books on designing polymermachinery with the help of computers. Prior to starting his consulting company in 198 7,he worked as a visiting professor at the Indian Institute of Technology, Chennai, India.Besides consultating, he also holds seminars, teaching the application of his software fordesigning extrusion and injection molding machinery.
He is currently giving lectures in polymer engineering at the University of Texas, in Austinand at the University of Massachusetts in Lowell, USA. Natti is a member of SPE andTAPPI, and has been presenting papers at the annual conferences of these societies forthe last 10 years.
Guenter Schumacher obtained his Ph. D. in Applied Mathematics from the University ofKarlsruhe and worked as a lecturer there for a number of years. He contributedsignificantly to the improvement of the software for robotics and quality control. He ispresently working at the innovation center of the European Commission in Brussels,Belgium.
N a t t i S . R a o
G u n t e r S c h u m a c h e r
D e s i g n F o r m u l a s
f o r P l a s t i c s E n g i n e e r s
2 n d E d i t i o n
HANSERHanser Publishers, Munich • Hanser Gardner Publications, Cincinnati
The Authors:Dr.-Ing. Natti S. Rao, 327 Route 216, Ghent, NY 12075, USADr. Gunter Schumacher, Am Bollerweg 6, 75045 Walzbachtal-Johlingen, Germany
Distributed in the USA and in Canada byHanser Gardner Publications, Inc.6915 Valley Avenue, Cincinnati, Ohio 45244-3029, USAFax: (513) 527-8801Phone: (513) 527-8977 or 1-800-950-8977Internet: http://www.hansergardner.com
Distributed in all other countries byCarl Hanser VerlagPostfach 86 04 20, 81631 Munchen, GermanyFax: +49 (89) 98 48 09Internet: http://www.hanser.de
The use of general descriptive names, trademarks, etc., in this publication, even if the former are not especiallyidentified, is not to be taken as a sign that such names, as understood by the Trade Marks and Merchandise MarksAct, may accordingly be used freely by anyone.
While the advice and information in this book are believed to be true and accurate at the date of going to press,neither the authors nor the editors nor the publisher can accept any legal responsibility for any errors oromissions that may be made. The publisher makes no warranty, express or implied, with respect to the materialcontained herein.
Library of Congress Cataloging-in-Publication DataRao, Natti S.Design formulas for plastics engineers.-- 2nd ed. / Natti S. Rao, Gunter Schumacher.p. cm.Includes bibliographical references and index.ISBN 1-56990-370-0 (pbk.)1. Plastics. I. Schumacher, Gunter. II. Title.TPl 140.R36 2004668.4-dc222004017192
Bibliografische Information Der Deutschen BibliothekDie Deutsche Bibliothek verzeichnet diese Publikation in der DeutschenNationalbibliografie;detaillierte bibliografische Daten sind im Internetiiber <http://dnb.ddb.de> abrufbar.ISBN 3-446-22674-5
All rights reserved. No part of this book may be reproduced or transmitted in any form or by any means,electronic or mechanical, including photocopying or by any information storage and retrieval system, withoutpermission in wirting from the publisher.
© Carl Hanser Verlag, Munich 2004Production Management: Oswald ImmelTypeset by Manuela Treindl, Laaber, GermanyCoverconcept: Marc Muller-Bremer, Rebranding, Munchen, GermanyCoverdesign: MCP • Susanne Kraus GbR, Holzkirchen, GermanyPrinted and bound by Druckhaus "Thomas Miintzer", Bad Langensalza, Germany
P r e f a c e
Today, designing of machines and dies is done to a large extent with the help of computerprograms. However, the predictions of theses programs do not always agree with thepractical results, so that there is a need to improve the underlying mathematical models.Therefore, knowledge of the formulas, on which the models are based and the limits oftheir applicability is necessary if one wants to develop a new program or improve onealready in use.
Often the plastics engineer has to deal with different fields of engineering. The search forthe appropriate equations in the various fields concerned can be time-consuming.A collection of formulas from the relevant fields and their applications, as given in thisbook, make it easier to write one's own program or to make changes in an existing programto obtain a better fit with the experiments.
It is often the case that different equations are given in the literature on plastics technologyfor one and the same target quantity. The practicing engineer is sometimes at a lossjudging the validity of the equations he encounters in the literature.
During his long years of activity as an R&D engineer in the polymer field at the BASF AGand other companies, Natti Rao tested many formulas published while solving practicalproblems. This book presents a summary of the important formulas and their appli-cations, which Natti Rao, in cooperation with the well-known resin and machinemanufacturers, successfully applied to solve design and processing problems.
The formulas are classified according to the fields, rheology, thermodynamics, heattransfer, and part design. Each chapter covers the relevant relations with worked-outexamples. A separate chapter is devoted to the practical equations for designing extrusionand injection molding equipment with detailed examples in metric units.
In addition, this work contains new, straightforward, practical relationships that havebeen developed and tested in recent years in solving design problems in the area ofextrusion and injection molding.
The topic of polymer machine design has been dealt with in several books. However, inthese books the know-how was presented in a way that the vast majority of plasticsengineers cannot easily apply it to the problems in their day-to-day work. By means ofthoroughly worked-out, practical examples this book elucidates the computationalbackground of designing polymer machinery in a manner which every engineer canunderstand and easily apply in daily practice.
We wish to express our thanks to our colleagues at the University of Massachusetts atLowell, USA, for fruitful discussions. Our thanks are also due to Faculty Innovation Centerof the University of Austin, Texas, USA, for help in preparing the manuscript.
Austin, USAKarlsruhe, Germany
Natti S. Rao, Ph. D.Gunter Schumacher, Ph. D.
A F i n a l W o r d
The aim of this book is to present the basic formulas of rheology, thermodynamics, heattransfer, and strength of materials applicable to plastics engineering and to show how,starting from these formulas, models for designing polymer processing equipment canbe developed.
Thoroughly worked out examples in metric units illustrate the use of these formulas,which have been successfully applied by well known machine manufacturers time andagain in their design work. However, owing to the ever increasing growth of knowledgebrought forth by research and development in the plastics field, a book of this kind needsto be renewed often and as such cannot claim to be an exhaustive work.
165 This page has been reformatted by Knovel to provide easier navigation.
Index
Index terms Links Index terms Links
A Absorption 70
B Bagley plot 6
Biot number 54 55 57 60
Brinkman number 60 140 142
Buckling 132
C Clamp force 139
Conduction 43 composite walls 46 cylinder 44 dissipation, with 59 hollow sphere 45 plane wall 43 sphere 45
Contact temperature 57
Convection resistance 49
Cooling channel 145 mechanical design 149
Cooling of melt 142 amorphous polymers 145
crystalline polymers 142 in mold 142
Cooling time 52 145
Correction factor 111
Critical strain 77
D Deborah number 60
Deflection 131
Desorption 69 70
Die geometry 81
Die swell 31
Dielectric heating 67
Diffusion coefficient 69
Dimensionless numbers 60
E Engineering strain 1
Enthalpy 38
Entrance loss 5
Extensional flow 31
Extrusion die 81
Extrusion screws 105
166 Index terms Links Index terms Links
This page has been reformatted by Knovel to provide easier navigation.
F Fick's Law 69
Findley function 77
Flight diameter 112
Flow curves 6
Flow length 156
Flowability 139
Fourier number 51 60
G Glass transition
temperature 41
Graetz number 60 140 142
Grashof number 60
H Half-life 70
Heat penetration 57
Heat transfer 43
Hencky strain 1
Hookean solid 2
Hooke's Law 3
Hyperbolic Function 8
I Ideal solid 1
L Lambert's law 65
Lewis number 60
Linear Viscoelastic Behavior 19 25
creep 26 tensile extensional flow 25
M Maxwell
fluid 30 model 29
Mechanical design of cooling channels 149
Mechanical design of extrusion screws 131
Melt conveying 109
Melt film 118
Melt pressure 116
Melt temperature 115
Melting injection molding
screws 150 parameter 121 profile 122 rate 121 screw rotation 151
Modulus of elasticity 3
N Nahme number 60
Newtonian Fluids 3
Non-Newtonian fluids 4
167 Index terms Links Index terms Links
This page has been reformatted by Knovel to provide easier navigation.
Nonlinear Viscoelastic Behavior 23 28
tensile compliance 28 tensile extensional flow 28 tensile relaxation
modulus 28 transient state 24
Nusselt number 60
P Part failure 74
Peclet number 60
Permeability 69
Plastics parts 73
Poisson ratio 2
Prandtl number 60 140
R Radiation 64
Recoverable shear strain 19
Reference area 2
Relative velocity 120
Retardation 20
Reynolds number 60 142
Runner 134
S Scale-up of screw
extruders 126
Schmidt number 60
Screw extruders mechanical design 131 scale-up 126
Shear 19 compliance 23 time-dependent behavior 20
Shear flow 4 steady 19
Shear rate 5 apparent 5
Shear Stress 6
Sherwood number 60
Shift factor 12
Solids conveying 105 conveying efficiency 106
Specific heat 36
Spiral melt flows 156
Stefan-Boltzmann constant 64
Stokes number 60
T Temperature fluctuation 125
Tensile creep compliance 26
Tensile stress 1
Thermal conductivity 40
Torsion 131
Trouton viscosity 4
168 Index terms Links Index terms Links
This page has been reformatted by Knovel to provide easier navigation.
V Viscosity
apparent 7 true 8
Viscosity function Carreau 14 Klein 16
Muenstedt 11 power law 9
Viscosity, influence of mixture 18 molecular weight 17 pressure 16 shear rate 8
vii This page has been reformatted by Knovel to provide easier navigation.
Contents
Preface ......................................................................................... v
1. Formulas of Rheology .......................................................... 1 1.1 Ideal Solids .................................................................................... 1
1.1.1 Hooke's Law ................................................................ 3 1.2 Newtonian Fluids ........................................................................... 3 1.3 Formulas for Viscous Shear Flow of Polymer Melts .................... 4
1.3.1 Apparent Shear Rate ................................................... 5 1.3.2 Entrance Loss .............................................................. 5 1.3.3 True Shear Stress ........................................................ 6 1.3.4 Apparent Viscosity ....................................................... 7 1.3.5 True Shear Rate .......................................................... 7 1.3.6 True Viscosity .............................................................. 8 1.3.7 Empirical Formulas for Apparent Viscosity ................... 8
1.3.7.1 Hyperbolic Function of Prandtl and Eyring ......... 8 1.3.7.2 Power Law of Ostwald and de Waele ................ 9 1.3.7.3 Muenstedt's Polynomial ..................................... 11 1.3.7.4 Carreau's Viscosity Equation ............................. 14 1.3.7.5 Klein’s Viscosity Formula ................................... 16 1.3.7.6 Effect of Pressure on Viscosity .......................... 16 1.3.7.7 Dependence of Viscosity on Molecular
Weight ................................................................ 17 1.3.7.8 Viscosity of Two Component Mixtures ............... 18
viii Contents
This page has been reformatted by Knovel to provide easier navigation.
1.4 Viscoelastic Behavior of Polymers ................................................ 18 1.4.1 Shear ........................................................................... 19
1.4.1.1 Linear Viscoelastic Behavior .............................. 19 1.4.1.2 Nonlinear Viscoelastic Behavior ........................ 23
1.4.2 Uniaxial Tension .......................................................... 25 1.4.2.1 Linear Viscoelastic Behavior .............................. 25 1.4.2.2 Nonlinear Viscoelastic Behavior ........................ 28
1.4.3 Maxwell Model ............................................................. 29 1.4.4 Practical Formulas for Die Swell and Extensional
Flow ............................................................................. 31
2. Thermodynamic Properties of Polymers ............................ 35 2.1 Specific Volume ............................................................................. 35 2.2 Specific Heat ................................................................................. 36 2.3 Enthalpy ......................................................................................... 38 2.4 Thermal Conductivity .................................................................... 40
3. Formulas of Heat Transfer ................................................... 43 3.1 Steady State Conduction .............................................................. 43
3.1.1 Plane Wall .................................................................... 43 3.1.2 Cylinder ....................................................................... 44 3.1.3 Hollow Sphere ............................................................. 45 3.1.4 Sphere ......................................................................... 45 3.1.5 Heat Conduction in Composite Walls ........................... 46 3.1.6 Overall Heat Transfer through Composite
Walls ............................................................................ 49 3.2 Transient State Conduction .......................................................... 50
3.2.1 Temperature Distribution in One-Dimensional Solids ........................................................................... 51
3.2.2 Thermal Contact Temperature ..................................... 57
Contents ix
This page has been reformatted by Knovel to provide easier navigation.
3.3 Heat Conduction with Dissipation ................................................. 59 3.4 Dimensionless Groups .................................................................. 60
3.4.1 Physical Meaning of Dimensionless Groups ................ 61 3.5 Heat Transfer by Convection ........................................................ 62 3.6 Heat Transfer by Radiation ........................................................... 64 3.7 Dielectric Heating .......................................................................... 67 3.8 Fick's Law of Diffusion ................................................................... 69
3.8.1 Permeability ................................................................. 69 3.8.2 Absorption and Desorption ........................................... 70
4. Designing Plastics Parts ...................................................... 73 4.1 Strength of Polymers ..................................................................... 73 4.2 Part Failure .................................................................................... 74 4.3 Time-Dependent Deformational Behavior .................................... 76
4.3.1 Short-Term Stress-Strain Behavior .............................. 76 4.3.2 Long-Term Stress-Strain Behavior ............................... 77
5. Formulas for Designing Extrusion and Injection Molding Equipment ............................................................... 81 5.1 Extrusion Dies ............................................................................... 81
5.1.1 Calculation of Pressure Drop ....................................... 81 5.1.1.1 Effect of Die Geometry on Pressure
Drop ................................................................... 81 5.1.1.2 Shear Rate in Die Channels .............................. 83 5.1.1.3 General Relation for Pressure Drop in Any
Given Channel Geometry .................................. 83 5.1.1.4 Examples ........................................................... 84 5.1.1.5 Temperature Rise and Residence Time ............ 94 5.1.1.6 Adapting Die Design to Avoid Melt
Fracture .............................................................. 95 5.1.1.7 Designing Screen Packs for Extruders .............. 102
x Contents
This page has been reformatted by Knovel to provide easier navigation.
5.2 Extrusion Screws ........................................................................... 105 5.2.1 Solids Conveying ......................................................... 105 5.2.2 Melt Conveying ............................................................ 109
5.2.2.1 Correction Factors ............................................. 111 5.2.2.2 Screw Power ...................................................... 111 5.2.2.3 Heat Transfer between the Melt and the
Barrel ................................................................. 114 5.2.2.4 Melt Temperature ............................................... 115 5.2.2.5 Melt Pressure ..................................................... 116
5.2.3 Melting of Solids .......................................................... 118 5.2.3.1 Thickness of Melt Film ....................................... 118 5.2.3.2 Melting Rate ....................................................... 121 5.2.3.3 Dimensionless Melting Parameter ..................... 121 5.2.3.4 Melting Profile .................................................... 122
5.2.4 Temperature Fluctuation of Melt .................................. 125 5.2.5 Scale-up of Screw Extruders ........................................ 126 5.2.6 Mechanical Design of Extrusion Screws ...................... 131
5.2.6.1 Torsion ............................................................... 131 5.2.6.2 Deflection ........................................................... 131
5.3 Injection Molding ........................................................................... 133 5.3.1 Pressure Drop in Runner ............................................. 134 5.3.2 Mold Filling .................................................................. 137
5.3.2.1 Injection Pressure and Clamp Force .................................................................. 137
5.3.3 Flowability of Injection Molding Resins ......................... 139 5.3.4 Cooling of Melt in Mold ................................................ 142
5.3.4.1 Crystalline Polymers .......................................... 142 5.3.4.2 Amorphous Polymers ......................................... 145
5.3.5 Design of Cooling Channels ......................................... 145 5.3.5.1 Thermal Design .................................................. 145 5.3.5.2 Mechanical Design ............................................. 149
Contents xi
This page has been reformatted by Knovel to provide easier navigation.
5.3.6 Melting in Injection Molding Screws ............................. 150 5.3.6.1 Melting by Heat Conduction ............................... 150 5.3.6.2 Melting during Screw Rotation ........................... 151
5.3.7 Predicting Flow Length of Spiral Melt Flows ................. 156
A Final Word ............................................................................... 163
Biography .................................................................................... 164
Index ............................................................................................ 165